# concrete mix design manualconcrete mix design …

Embed Size (px)

TRANSCRIPT

Final BOOK NEWlar domie pdf copy.cdrCONCRETE MIX DESIGN
MANUALCONCRETE MIX DESIGN MANUALCONCRETE MIX DESIGN MANUALCONCRETE
MIX DESIGN MANUALCONCRETE MIX DESIGN MANUALCONCRETE MIX DESIGN
MANUAL

FIRST EDITION: AUGUST 2017

SPECIAL PUBLICATION NO. COREN/2017/016/RC

CONCRETE MIX DESIGN MANUAL

ENGINEERING IN NIGERIA

ENGINEERING IN NIGERIA

1. Engr. Prof. Charles Uko, FNSE Chairman University of Uyo

2. Engr. K.A Ali, FNSE, NPOM, mni COREN

3. Engr. W. Kamila Maliki, FNSE, mni COREN

4. Engr. M.U. Adoyi, FNSE COREN

5. Engr. A. J. Agabi, MNSE COREN

6. Engr. Lukman Sani, MNSE COREN

7. Engr. Ahmed A.S.Y. Kutigi, MNSE COREN

8. Engr. Prof. Danladi S. Matawal, MNSE NBBRI

9. Engr. (Mrs. Emeso B. Ojo, MNSE NBBRI

10. Engr. Gai F. Iliya, MNSE NBBRI

11. Mr. George Omange NBBRI

12. Engr. Bukola S. Adebisi, MNSE LAFARGE

13. Dr. Abdullahi S.B. Gimba LAFARGE

14. Mr. Vipul Agrawal LAFARGE

15. Engr. Femi Yusuf, MNSE LAFARGE

16. Engr. M.I. Nwoye, FNSE JULIUS BERGER

17. Engr. Joern Seitz JULIUS BERGER

18. Engr. Mustapha Olu JULIUS BERGER

19. Mr. M. Jagdish DANGOTE

20. Engr. Ben Ani NSE

ii

S/N NAME/ INTEREST INSTITUTION

1. Engr. Prof. Charles Uko, MNSE Chairman Council for the Regulation of Engineering in Nigeria.

2. Engr. Kashim A. Ali, FNSE, NPOM, mni Council for the Regulation of Engineering in Nigeria.

3. Engr. Kamila W. Maliki, FNSE, mni Council for the Regulation of Engineering in Nigeria.

4. Engr. M.U. Adoyi, FNSE Council for the Regulation of Engineering in Nigeria.

5. Engr. A. J. Agabi, MNSE Council for the Regulation of Engineering in Nigeria.

6. Engr. Lukman Sani, MNSE Council for the Regulation of Engineering in Nigeria.

7. Engr. Ahmed A.S.Y. Kutigi, MNSE Council for the Regulation of Engineering in Nigeria.

8. Engr. Prof. Danladi S. Matawal, MNSE Nigeria Building and Road Research Institute.

9. Engr. (Mrs.) Emeso B. Ojo, MNSE Nigeria Building and Road Research Institute.

10. Engr. Gai F. Iliya, MNSE Nigeria Building and Road Research Institute.

11. Mr. George Omange Nigeria Building and Road Research Institute.

12. Engr. Ben Ani Nigerian Society of Engineers.

13. Engr. M.I. Nwoye, FNSE Julius Berger Nigeria Plc.

14. Engr. Joern Seitz Julius Berger Nigeria Plc.

15. Engr. Mustapha Olu Julius Berger Nigeria Plc.

16. Mr. M. Jagdish Dangote Cement Plc.

17. Engr. Bukola S. Adebisi, MNSE Lafarge Africa Plc.

18. Mr. Vipul Agrawal Lafarge Africa Plc.

19. Engr. Femi Yusuf, MNSE Lafarge Africa Plc.

iii

FOREWORD

It is with deep sense of joy that the Council for the Regulation of Engineering in Nigeria, COREN, present the Concrete Mix Design Manual for Nigeria. This is indeed historic, as sad as it is, we must admit that this is the first of its type as the nation had never had her own Concrete Mix Design Manual. Like in many areas of our national life, we had all these years depended on the Concrete Mix Design Manual of other nations irrespective of their sharp differences in their environmental and other factors.

The challenge was heightened when in 2014, controversies became pervasive as to classes and qualities of cement. Eventhough the issues on the subject were promptly put to rest with the conclusion that cement classification does not cause building collapse but rather its application.

This, and the need to take up a national industry challenge, compelled COREN to commence the project of producing the Concrete Mix Design Manual for Nigeria.

The journey has been chequered with various challenges all of which were proficiently surmounted in the course of the project.

It started with the formation of a Technical Committee with membership carefully selected from the academia and the industry. The work of the Committee included laboratory tests, the results of which were variously subjected to further confirmation tests carried out in various Universities in the geo-political zones of Nigeria. The work was further subjected to critique analysis to arrive at a document that has no doubt, met international standard and the test of time.

The Concrete Mix Design Manual for Nigeria, like any document of this nature must be subjected to periodic review. Every reference document goes obsolete if left to drift for eternity, that is, without review.

The Manual, for practitioners in Nigeria using concrete, must now replace the foreign manuals which has produced the danger of non-uniformity because of diverse sources. The Concrete Mix Design Manual for Nigeria, therefore, provides homogeneity for all concrete design.

In the application of this manual, a trial mix is mandatory for any major construction site in Nigeria.

On behalf of the COREN, I wish to express my profound appreciation to the Chairman and members of the Technical Committee, the various construction companies which readily gave their support to this project, the Universities which made their laboratories and personnel available, the Management and staff of the Nigerian Building and Road Research Institute, NBRRI, Lafarge Cement, Dangote Cement and those of COREN who committed so much of their time and energy to this project.

This is indeed a historic achievement but opening the window of challenges in our need to develop our indigenous Codes and standards as we take Engineering Practice to higher levels in Nigeria.

Engr. Kashim A. Ali, FNSE, mni

President, COREN

iii

FOREWORD

It is with deep sense of joy that the Council for the Regulation of Engineering in Nigeria, COREN, present the Concrete Mix Design Manual for Nigeria. This is indeed historic, as sad as it is, we must admit that this is the first of its type as the nation had never had her own Concrete Mix Design Manual. Like in many areas of our national life, we had all these years depended on the Concrete Mix Design Manual of other nations irrespective of their sharp differences in their environmental and other factors.

The challenge was heightened when in 2014, controversies became pervasive as to classes and qualities of cement. Eventhough the issues on the subject were promptly put to rest with the conclusion that cement classification does not cause building collapse but rather its application.

This, and the need to take up a national industry challenge, compelled COREN to commence the project of producing the Concrete Mix Design Manual for Nigeria.

The journey has been chequered with various challenges all of which were proficiently surmounted in the course of the project.

It started with the formation of a Technical Committee with membership carefully selected from the academia and the industry. The work of the Committee included laboratory tests, the results of which were variously subjected to further confirmation tests carried out in various Universities in the geo-political zones of Nigeria. The work was further subjected to critique analysis to arrive at a document that has no doubt, met international standard and the test of time.

The Concrete Mix Design Manual for Nigeria, like any document of this nature must be subjected to periodic review. Every reference document goes obsolete if left to drift for eternity, that is, without review.

The Manual, for practitioners in Nigeria using concrete, must now replace the foreign manuals which has produced the danger of non-uniformity because of diverse sources. The Concrete Mix Design Manual for Nigeria, therefore, provides homogeneity for all concrete design.

In the application of this manual, a trial mix is mandatory for any major construction site in Nigeria.

On behalf of the COREN, I wish to express my profound appreciation to the Chairman and members of the Technical Committee, the various construction companies which readily gave their support to this project, the Universities (especially the University of Uyo, Uyo) which made their laboratories and personnel available, the Management and staff of the Nigerian Building and Road Research Institute, NBRRI, Lafarge Cement, Dangote Cement and those of COREN who committed so much of their time and energy to this project.

This is indeed a historic achievement but opening the window of challenges in our need to develop our indigenous Codes and standards as we take Engineering Practice to higher levels in Nigeria.

Engr. Kashim A. Ali, FNSE, mni

President, COREN August, 2017

Council for the Regulation of Engineering in Nigeria i

Technical Team ii

1.3. Requirements of Concrete Mix Design 1

1.4. Variability of Concrete Strength 2 - 3

1.5. Selecting Mix Characteristics 3

1.6. Decision Variables in Mix Design 3

1.6.1 Water Cement ratio 3

1.6.2 Cement Content 3

1.7.1 Compressive Strength 4

2.2. AGREGATES 6

2.2.3 Shape and Texture 6 - 7

PART TWO: NIGERIAN CEMENT, AGGREGATE, ADMIXTURE AND

CONCRETE STANDARDS

Council for the Regulation of Engineering in Nigeria i

Technical Team ii

1.3. Requirements of Concrete Mix Design 1

1.4. Variability of Concrete Strength 2 - 3

1.5. Selecting Mix Characteristics 3

1.6. Decision Variables in Mix Design 3

1.6.1 Water Cement ratio 3

1.6.2 Cement Content 3

1.7.1 Compressive Strength 4

2.2. AGREGATES 6

2.2.3 Shape and Texture 6 - 7

PART TWO: NIGERIAN CEMENT, AGGREGATE, ADMIXTURE AND

CONCRETE STANDARDS

2.2.7 Maximum Nominal Size of Aggregate 7 - 8

2.2.8 Grading and Type of Aggregate 8

2.3. ADMIXTURES 8

2.3.2. Chemical Admixtures 8

2.4. CONCRETE GRADES 9

3.1. Introduction to mix design 10

3.2. Determination of Target Mean Strength 10

3.3. Determination of Water-Cement ratio 10 - 11

3.4. Determination of Water content 12

3.5. Determination of cement content 12

3.6. Determination of aggregate content 12 - 13 3.7. Trial Mixes 13 - 15

v

2.2.7 Maximum Nominal Size of Aggregate 7 - 8

2.2.8 Grading and Type of Aggregate 8

2.3. ADMIXTURES 8

2.3.2. Chemical Admixtures 8

2.4. CONCRETE GRADES 9

3.1. Introduction to mix design 10

3.2. Determination of Target Mean Strength 10

3.3. Determination of Water-Cement ratio 10 - 11

3.4. Determination of Water content 12

3.5. Determination of cement content 12

3.6. Determination of aggregate content 12 - 13 3.7. Trial Mixes 13 - 15

3.8. Worked examples 15 - 18

v

LIST OF TABLES

Table1: Strength ranges for various grades of cement in use in Nigeria.

Table 2: Aggregate properties and its influence on concrete performance.

Table 3: Impact of aggregates shape and texture in concrete.

Table 4: Strength Classes of Concrete according to EN 206-1

Table 5: Approximate Free water contents required to give various levels of workability

LIST OF FIGURES

Fig 2 Grading Curve for 5-15 Coarse Aggregate

Fig 3 Strength versus water/cement Ratio for Nigeria Cements

Fig 4.1 Combined aggregate curves for curves for fine sand and 5-15 coarse

aggregate.

Fig 4.2 Combined aggregate curves for curves for fine sand and 10-15 coarse

aggregate.

Fig 4.3 Combined aggregate grading curve for 21% fine and 79% coarse

Fig 4.4 Combined aggregate grading curve for 21% fines and 79% coarse using

COMBAG16

vi

LIST OF TABLES

Table1: Strength ranges for various grades of cement in use in Nigeria.

Table 2: Aggregate properties and its influence on concrete performance.

Table 3: Impact of aggregates shape and texture in concrete.

Table 4: Strength Classes of Concrete according to EN 206-1

Table 5: Approximate Free water contents required to give various levels of workability

LIST OF FIGURES

Fig 2 Grading Curve for 5-15 Coarse Aggregate

Fig 3 Strength versus water/cement Ratio for Nigeria Cements

Fig 4.1 Combined aggregate curves for curves for fine sand and 5-15 coarse

aggregate.

Fig 4.2 Combined aggregate curves for curves for fine sand and 10-15 coarse

aggregate.

Fig 4.3 Combined aggregate grading curve for 21% fine and 79% coarse

Fig 4.4 Combined aggregate grading curve for 21% fines and 79% coarse using

COMBAG16

vi

CONCRETE MIX DESIGN MANUAL

1.1. Scope This manual provides guidelines for the determination of the appropriate concrete mixes required for various construction applications. It provides a step by step procedure required for deducing the appropriate quantities of constituents required to achieve concrete with specified characteristics in accordance to EN 206. This manual is applicable for designing concrete mixes using Portland Limestone Cements conforming to NIS 444-1 and natural aggregates in conformity to EN 12620. With the advent of various strength classes of cement for construction, it is now possible to use any strength class of cement to obtain concrete of a specified characteristic strength provided the mix design is carried out appropriately. This mix design manual sets out the guidelines for concrete mixes in Nigeria.

1.2. Concept of Mix Design Concrete can be designed for strength ranging from 10MPa to 100MPa(note that

2 MPa is used instead of N/mm throughout this manual)making it an extremely versatile building material. In all these cases, the basic constituents remain the same, but it is their relative proportions that determine the properties.

In designing a concrete mix, the primary objective is to select suitable constituent materials and determine their required amounts in order to produce concrete of specific characteristics and properties as economically as possible. The characteristics typically specified are workability, strength and durability. Other characteristics that may be required includes; density, thermal characteristics, elastic modulus etc.

However, the mix design process only considers the factors which have a major effect on the properties of concrete i.e. workability, strength and durability. The proportioning of the constituent materials of concrete is dependent on the required performance of concrete in two states: the fresh/plastic and hardened states. Four variable factors need to be considered in mix proportioning:

i. Water-cement ratio ii. Cement content iii. Gradation of aggregates iv. Consistency

Typically, two or three factors are specified and the others are adjusted to achieve minimum workability and economy. In summary, the goal of mix proportioning is to use the minimum quantity of cement that will lubricate the mixture when fresh to allow for adequate placing and at the same time, bind the aggregates together and fill up the voids between them when the concrete has hardened. Any excess of paste results in a higher cost, higher drying shrinkage.

1.3. Requirements of Concrete Mix Design At the mix design stage, available data for deriving the required proportions of constituent materials is usually limited. The data provided in this manual are estimates and should be replaced where there is more appropriate data with regards to the local materials.

Part one: Introduction to Concrete Mix Design

1

CONCRETE MIX DESIGN MANUAL

1.1. Scope This manual provides guidelines for the determination of the appropriate concrete mixes required for various construction applications. It provides a step by step procedure required for deducing the appropriate quantities of constituents required to ach ieve concre te wi th spec i f i ed characteristics in accordance to EN 206. This manual is applicable for designing concrete mixes using Portland Limestone Cements conforming to NIS 444-1 and natural aggregates in conformity to EN 12620. With the advent of various strength classes of cement for construction, it is now possible to use any strength class of cement to obtain concrete of a specified characteristic strength provided the mix design is carried out appropriately. This mix design manual sets out the guidelines for concrete mixes in Nigeria.

1.2. Concept of Mix Design Concrete can be designed for strength ranging from 10MPa to 100MPa(note that MPa is used

2instead of N/mm throughout th is manual)making it an extremely versatile building material. In all these cases, the basic constituents remain the same, but it is their relative proportions that determine the properties.

In designing a concrete mix, the primary objective is to select suitable constituent materials and determine their required amounts in order to produce concrete of specific characteristics and properties as economically as possible. The characteristics typically specified are workability, strength and durability. Other characteristics that may be required includes; density, thermal characteristics, elastic modulus etc.

However, the mix design process only considers the factors which have a major effect on the properties of concrete i.e. workability, strength and durability. The proportioning of the

constituent materials of concrete is dependent on the required performance of concrete in two states: the fresh/plastic and hardened states. Four variable factors need to be considered in mix proportioning:

i. Water-cement ratio ii. Cement content iii. Gradation of aggregates iv. Consistency

Typically, two or three factors are specified and the others are adjusted to achieve minimum workability and economy. In summary, the goal of mix proportioning is to use the minimum quantity of cement that will lubricate the mixture when fresh to allow for adequate placing and at the same time, bind the aggregates together and fill up the voids between them when the concrete has hardened. Any excess of paste results in a higher cost, higher drying shrinkage.

1.3. Requirements of Concrete Mix Design At the mix design stage, available data for deriving the required proportions of constituent materials is usually limited. The data provided in this manual are estimates and should be replaced where there is more appropriate data with regards to the local materials.

Part one: Introduction to Concrete Mix Design

1

Mean Strength

The necessary data required can be classified

into two categories viz a viz: a. Specified variables: These are variables which are normally selected in the specifications based on intended use of the concrete. They include:

· The minimum compressive strength

concrete

available compaction equipment

· Maximum water-cement ratio

· Maximum/minimum cement content

· Strength class of cement

· Maximum aggregate size

b. Additional information: This refers to data on the available materials required for the concrete mix. They include: · The standard deviation which is a measure of the variability from the specified characteristic strength · The type of aggregate · Specific gravity of aggregate · Grading of fine aggregate

Understanding the basic concept of mix design is as significant as the actual calculations required for determining the mix proportions. In fact, the appropriate mix proportions are a consequence of the concrete mix design.

1.4. Variability of Concrete Strength In the production of concrete, there are inevitable variations in the properties of the

materials used as well as the construction methods. For instance, the quality of various batches of cement supplied may vary, or the grading and particle shape of the aggregates may vary. These variations may even be observed within a batch as a result of process of sampling, production, curing and testing of specimens even if they are conducted in accordance with the recommended standard. This results in variation of strength from batch to batch and also within a batch. This makes the strength of the final product difficult to assess.

In concrete mix design, it is now generally accepted that the variation in concrete strengths follow the normal distribution curve shown in Figure 1.1. The area under the curve represents the total number of test results. If a vertical line is drawn through a specified value, the proportion of results less than that value is represented by the area beneath the curve and to the left hand side of the vertical line as demonstrated in Figure 1.1. The normal distribution curve is defined by two parameters: its mean and standard deviation. The curve is symmetrical about its mean and the standard deviation is a measure of the variability. Typically at a given level of quality control, the standard deviation increases as the specified characteristic strength.

2

Mean Strength

The necessary data required can be classified

into two categories viz a viz: a. Specified variables: These are variables which are normally selected in the specifications based on intended use of the concrete. They include:

· The minimum compressive strength

concrete

available compaction equipment

· Maximum water-cement ratio

· Maximum/minimum cement content

· Strength class of cement

· Maximum aggregate size

b. Additional information: This refers to data on the available materials required for the concrete mix. They include: · The standard deviation which is a measure of the variability from the specified characteristic strength · The type of aggregate · Specific gravity of aggregate · Grading of fine aggregate

Understanding the basic concept of mix design is as significant as the actual calculations required for determining the mix proportions. In fact, the appropriate mix proportions are a consequence of the concrete mix design.

1.4. Variability of Concrete Strength In the production of concrete, there are inevitable variations in the properties of the

materials used as well as the construction methods. For instance, the quality of various batches of cement supplied may vary, or the grading and particle shape of the aggregates may vary. These variations may even be observed within a batch as a result of process of sampling, production, curing and testing of specimens even if they are conducted in accordance with the recommended standard. This results in variation of strength from batch to batch and also within a batch. This makes the strength of the final product difficult to assess.

In concrete mix design, it is now generally accepted that the variation in concrete strengths follow the normal distribution curve shown in Figure 1.1. The area under the curve represents the total number of test results. If a vertical line is drawn through a specified value, the proportion of results less than that value is represented by the area beneath the curve and to the left hand side of the vertical line as demonstrated in Figure 1.1. The normal distribution curve is defined by two parameters: its mean and standard deviation. The curve is symmetrical about its mean and the standard deviation is a measure of the variability. Typically at a given level of quality control, the standard deviation increases as the specified characteristic strength.

2

CONCRETE MIX DESIGN MANUAL

This statistical quality control method prov ides a sc ient i f i c approach to understanding the variations that are encountered on site so as to provide proper tolerance to allow for inevitable variations. To obtain the standard deviation on site, the minimum number of test samples should be between 20 to 30. The standard deviation used for any calculation should be based on either result obtained from the site, or in the absence of such data, assumed values are specified in different standards. Most producers of concrete in Nigeria do not have the quality control ability to have small standard deviations. To this end it is suggested that producers without adequate records start with a standard deviation of 6MPa, if thereafter a consecutive result of 30 tests is available, the standard deviation should be based on the result from the 30 consecutive tests. Whenever the producer is convinced that he can achieve a lower standard deviation, he can use that new value for mix design. 1.5. Selecting Mix Characteristics

The primary objective of the mix design is to

achieve the specified properties in the most

economical manner.

materials and mixture characteristics can the

specified properties be obtained in concrete

construction. As a result, adequate knowledge

of the constituent material properties and

properties of concrete in the plastic condition

is a prerequisite for a proper mix design. Also,

the exposure conditions and the intended use

of the concrete are also factored in whilst

carrying out the mix design as the

characteristics of the concrete should reflect

the needs of the structure.

Once the required characteristics have been

selected, the mixture is proportioned using data obtained from the field or the laboratory to achieve the specified requirements.

1.6. Decision Variables in Mix Design

The following are the key decision variables

when estimating the proportions in a concrete

mix:

important parameter that determines the

strength and durability of concrete. The

strength of concrete is dependent on the

water cement ratio and not totally on the

cement content. According to Abram's law,

the higher the water cement ratio, the lower

the strength of concrete. It is generally

accepted as a rule of thumb that every 1%

increase in quantity of water added reduces

the strength of concrete by 5%. Theoretically,

a water cement ratio of 0.25 is required for the

complete hydration of cement. Hence, it is

very important to control the water cement

ratio on site.

1.6.2. Cement Content Cement is the binder material in concrete which imparts strength to the concrete. With regards to durability, conditions of exposure govern the maximum cement contents required. For a given workability, a certain water content is required. This implies that a higher cement content would be required to achieve a desired workability at a lower water cement ratio. Based on the relationship between cement content and water cement ratio, we see that a greater water cement ratio would require a lower cement content. Details

3

CONCRETE MIX DESIGN MANUAL

This statistical quality control method provides a scientific approach to understanding the variations that are encountered on site so as to provide proper tolerance to allow for inevitable variations. To obtain the standard deviation on site, the minimum number of test samples should be between 20 to 30. The standard deviation used for any calculation should be based on either result obtained from the site, or in the absence of such data, assumed values are specified in different standards. Most producers of concrete in Nigeria do not have the quality control ability to have small standard deviations. To this end it is suggested that producers without adequate records start with a standard deviation of 6MPa, if thereafter a consecutive result of 30 tests is available, the standard deviation should be based on the result from the 30 consecutive tests. Whenever the producer is convinced that he can achieve a lower standard deviation, he can use that new value for mix design. 1.5. Selecting Mix Characteristics

The primary objective of the mix design is to

achieve the specified properties in the most

economical manner.

materials and mixture characteristics can the

specified properties be obtained in concrete

construction. As a result, adequate knowledge

of the constituent material properties and

properties of concrete in the plastic condition is

a prerequisite for a proper mix design. Also, the

exposure conditions and the intended use of the

concrete are also factored in whilst carrying out

the mix design as the characteristics of the

concrete should reflect the needs of the

structure.

Once the required characteristics have been

selected, the mixture is proportioned using data obtained from the field or the laboratory to achieve the specified requirements.

1.6. Decision Variables in Mix Design

The following are the key decision variables

when estimating the proportions in a concrete

mix:

important parameter that determines the

strength and durability of concrete. The

strength of concrete is dependent on the water

cement ratio and not totally on the cement

content. According to Abram's law, the higher

the water cement ratio, the lower the strength of

concrete. It is generally accepted as a rule of

thumb that every 1% increase in quantity of

water added reduces the strength of concrete by

5%. Theoretically, a water cement ratio of 0.25 is

required for the complete hydration of cement.

Hence, it is very important to control the water

cement ratio on site.

1.6.2. Cement Content Cement is the binder material in concrete which imparts strength to the concrete. With regards to durability, conditions of exposure govern the maximum cement contents required. For a given workability, a certain water content is required. This implies that a higher cement content would be required to achieve a desired workability at a lower water cement ratio. Based on the relationship between cement content and water cement ratio, we see that a greater water cement ratio would require a lower cement content. Details on properties and types of cement and how they relate to concrete properties are presented in chapter two of this manual.

1.6.3. Relative Proportion of Aggregates

Aggregates in concrete are of two types:

3

CONCRETE MIX DESIGN MANUAL

Coarse aggregates which refer to materials retained on 4.75mm sieve size; and Fine aggregates which are materials passing through 4.75mm sieve size. The proportion of fine aggregates to coarse aggregate in a concrete mix depend on the fineness of the fine aggregate, size/shape of coarse aggregates and the cement content. Details of the effect of properties of aggregates on properties of concrete mixes are presented in chapter three

1.7. Factors Affecting Concrete Mix Pro- portions The process of designing a concrete mix consists of selecting the appropriate proportions of cement, fine aggregate, coarse aggregate and water to produce concrete having specified properties. The most fundamental way of specifying mix proportions is in terms of the mass of material in a unit volume of fully compacted concrete. The various factors affecting the choice of mix proportions include:

1.7.1. Compressive Strength The compressive strength of concrete is the most universally used measure for concrete quality. It influences other properties of hardened concrete. Studies have shown that the compressive strength of concrete is inversely proportional to the water cement ratio within practical limit. The strength of the cement paste binder in concrete is dependent on the quality and quantity of the reaction of the paste components and the extent to which the hydration reaction has progressed. The strength of concrete increases with time as

long as there is sufficient hydration water/moisture at a favorable temperature. Hence, the strength at a particular age is dependent on both the original water- cement ratio as well as the degree to which the cementitious materials have hydrated. The mean compressive strength at a specific age, typically 28 days, determines the water- cement ratio of the mix. (Except in pozolanic cement where ages 56 to 90 days may be specified)

1.7.2. Workability The workability required for various types of construction is dependent on various factors. The Slump test is typically used to determine the degree of workability. For a given proportion of cement and aggregates, the higher the slump, the wetter the mixture and higher the workability.

1.7.3. Durability Typically, high strength concrete is generally more resistant to adverse conditions as compared to low strength concrete. However, in conditions where high strength is not required but the concrete would be exposed to adverse conditions, the durability requirement will determine the water-cement ratio to be used. See EN 206-1 Concrete - Part 1: Specification, performance, production and Conformity.

4

CONCRETE MIX DESIGN MANUAL

Coarse aggregates which refer to materials retained on 4.75mm sieve size; and Fine aggregates which are materials passing through 4.75mm sieve size. The proportion of fine aggregates to coarse aggregate in a concrete mix depend on the fineness of the fine aggregate, size/shape of coarse aggregates and the cement content. Details of the effect of properties of aggregates on properties of concrete mixes are presented in chapter three

1.7. Factors Affecting Concrete Mix Pro- portions The process of designing a concrete mix consists of selecting the appropriate proportions of cement, fine aggregate, coarse aggregate and water to produce concrete having specified properties. The most fundamental way of specifying mix proportions is in terms of the mass of material in a unit volume of fully compacted concrete. The various factors affecting the choice of mix proportions include:

1.7.1. Compressive Strength The compressive strength of concrete is the most universally used measure for concrete quality. It influences other properties of hardened concrete. Studies have shown that the compressive strength of concrete is inversely proportional to the water cement ratio within practical limit. The strength of the cement paste binder in concrete is dependent on the quality and quantity of the reaction of the paste components and the extent to which the hydration reaction has progressed. The strength of concrete increases with time as

long as there is sufficient hydration water/moisture at a favorable temperature. Hence, the strength at a particular age is dependent on both the original water- cement ratio as well as the degree to which the cementitious materials have hydrated. The mean compressive strength at a specific age, typically 28 days, determines the water- cement ratio of the mix. (Except in pozolanic cement where ages 56 to 90 days may be specified)

1.7.2. Workability The workability required for various types of construction is dependent on various factors. The Slump test is typically used to determine the degree of workability. For a given proportion of cement and aggregates, the higher the slump, the wetter the mixture and higher the workability.

1.7.3. Durability Typically, high strength concrete is generally more resistant to adverse conditions as compared to low strength concrete. However, in conditions where high strength is not required but the concrete would be exposed to adverse conditions, the durability requirement will determine the water-cement ratio to be used. See EN 206-1 Concrete - Part 1: Specification, performance, production and Conformity.

4

Cement - Part 1: Composition, specifications

and conformity criteria for common cements.

This standard defines 27 product in the family

of common cement that are grouped into 5

main types.

Nigeria are Portland Limestone Cements which

is in the CEM II class of cement as defined in

NIS 444-1. This cement composes of limestone

as a blended addition to clinker and gypsum.

The above table presents the following facts

that should be of interest to the user of

concrete products:

contain cement whose strength at 28days is

higher than that contained in a bag labeled

Grade 42.5 because of the overlap of the

strength of the two grades between 32.5MPa

and 42.5MPa. What one can then safely say is

that the cement in a Grade 32.5 bag has strength

of not less than 32.5MPa. Similarly, one can also

say that the cement in a Grade 42.5 bag has

strength of not less than 42.5MPa. This is

important in that those not familiar with this

fact could jump to the false conclusion that a

particular cement is substandard;

contain cement whose strength at 28days is

higher than that contained in a bag labeled

Grade 52.5 because of the overlap of the

strength of the two grades between 52.5MPa

and 62.5MPa. What one can then safely say is

that the cement in a Grade 42.5 bag has strength

of not less than 42.5MPa. Similarly, one can also

say that the cement in a Grade 52.5 bag has

strength of not less than 52.5MPa.

This is a very important issue to remember

when dealing with cements under this new

standard. It should therefore be noted that the

actual strength of cement in any bag can only be

determined by test – not from the label on the

bag. The label only guarantees minimum

strength, but a concrete mix design ensures the

use of the actual cement strength.

2.1.1. Strength Classes of Cement

The strength classes of cement (i.e 32.5 MPa or

42.5MPa) refer to the minimum strength of

cement mortar after 28 days curing and testing

as per standard conditions as specified in the

NIS 445:2003. The relationship between

compressive strength and water cement ratio

has been established as a set of curves for the

various strength classes of cement. Various

types and strength of classes of cements require

varying water contents to produce pastes of

standard consistency. Hence the water-cement

ratio required to achieve the target mean

strength is also dependent on the strength class

of cement. A higher strength

Part Two: Nigerian Cement, Aggregate, Admixture And Concrete Standards

32.5

32.5R

42.5

42.5R

52.5

52.5R

MM

Table 1 shows the strengths of various cements available in Nigeria.

5

Cement - Part 1: Composition, specifications

and conformity criteria for common cements.

This standard defines 27 product in the family

of common cement that are grouped into 5

main types.

Nigeria are Portland Limestone Cements which

is in the CEM II class of cement as defined in

NIS 444-1. This cement composes of limestone

as a blended addition to clinker and gypsum.

The above table presents the following facts

that should be of interest to the user of

concrete products:

contain cement whose strength at 28days is

higher than that contained in a bag labeled

Grade 42.5 because of the overlap of the

strength of the two grades between 32.5MPa

and 42.5MPa. What one can then safely say is

that the cement in a Grade 32.5 bag has strength

of not less than 32.5MPa. Similarly, one can also

say that the cement in a Grade 42.5 bag has

strength of not less than 42.5MPa. This is

important in that those not familiar with this

fact could jump to the false conclusion that a

particular cement is substandard;

contain cement whose strength at 28days is

higher than that contained in a bag labeled

Grade 52.5 because of the overlap of the

strength of the two grades between 52.5MPa

and 62.5MPa. What one can then safely say is

that the cement in a Grade 42.5 bag has strength

of not less than 42.5MPa. Similarly, one can also

say that the cement in a Grade 52.5 bag has

strength of not less than 52.5MPa.

This is a very important issue to remember

when dealing with cements under this new

standard. It should therefore be noted that the

actual strength of cement in any bag can only be

determined by test – not from the label on the

bag. The label only guarantees minimum

strength, but a concrete mix design ensures the

use of the actual cement strength.

2.1.1. Strength Classes of Cement

The strength classes of cement (i.e 32.5 MPa or

42.5MPa) refer to the minimum strength of

cement mortar after 28 days curing and testing

as per standard conditions as specified in the

NIS 445:2003. The relationship between

compressive strength and water cement ratio

has been established as a set of curves for the

various strength classes of cement. Various

types and strength of classes of cements require

varying water contents to produce pastes of

standard consistency. Hence the water-cement

ratio required to achieve the target mean

strength is also dependent on the strength class

of cement. A higher strength

Part Two: Nigerian Cement, Aggregate, Admixture And Concrete Standards

32.5

32.5R

42.5

42.5R

52.5

52.5R

MM

Table 1 shows the strengths of various cements available in Nigeria.

5

Based on the relationship between compressive

strength of concrete and the water to cement

ratio for the various cement classes, it can be

deduced that a lower water to cement ratio

would be required to produce a concrete of a

specific characteristic strength when using a

lower strength class of cement. That is to say, a

specified grade of concrete can be produced

using any strength class of cement provided the

mix design procedure is followed.

2.2. AGGREGATES Aggregates are the main constituents of concrete because they do not only give the body to the concrete, but they also have a significant effect on the properties of fresh and hardened concrete based on their shape, size, texture, grading and crushing value.

The overall mechanical property of concrete depends on certain properties of aggregates itself. These aggregate properties include the source of aggregates, size of aggregate, shape of aggregate, crushing type of aggregates, angularity index, surface texture, modulus of elasticity, bulk density, specific gravity, absorption and moisture content, grading of aggregates. For a good concrete mix, aggregates need to be clean, hard, and strong with the particles free of absorbed chemicals or coatings of clay and other fine materials that are likely to interfere with the process of hydration.

2.2.1. Types of Aggregates

Aggregate characteristics have a significant effect on the behavior of fresh and hardened p rope r t i e s o f conc r e t e . Ag g r eg a t e

characteristics are function of particle size and as such, the following classification is used in accordance to common practice: material retained in the No.4 sieve (4.75mm) is considered as coarse aggregate; material passing No.4 sieve (4.75mm) and retained in the No. 200 sieve (75μm) is considered as fine aggregate; and material passing No. 200 sieve is referred to as micro-fines.

2.2.2. Properties of Aggregates

The main characteristics of aggregate that affect the performance of fresh and hardened concrete, even though some variation in aggregate properties is expected, are as follows:

2.2.3. Shape and Texture The shape and texture of both coarse and fine aggregates play a significant role in the properties fresh and hardened concrete. The shape and texture of coarse aggregate play an important role on the behavior of fresh and hardened concrete as they affect the demand for fine aggregate.

Flaky and elongated particles should be limited to between 35 to 40 percent, or the shape coefficient determined by Equation 3.1 which should not be less than 0.20.

where is the volume of particle I

is the size of particle I

High voids, Poor Bond Grip, Bleeding.

Good Bond Grip

Increase segregation, Finishing

Elongated

Rough

Water Demand.

Table 3: Impact of aggregates shape and texture in concrete.

Properties

Influence on Concrete Performance

Bonding, Water Demand, Absorption

Cohension, Water Demand (Strength)

Table 2: Aggregate properties and its influence on concrete performance.

Strength, Water demand

Based on the relationship between compressive

strength of concrete and the water to cement

ratio for the various cement classes, it can be

deduced that a lower water to cement ratio

would be required to produce a concrete of a

specific characteristic strength when using a

lower strength class of cement. That is to say, a

specified grade of concrete can be produced

using any strength class of cement provided the

mix design procedure is followed.

2.2. AGGREGATES Aggregates are the main constituents of concrete because they do not only give the body to the concrete, but they also have a significant effect on the properties of fresh and hardened concrete based on their shape, size, texture, grading and crushing value.

The overall mechanical property of concrete depends on certain properties of aggregates itself. These aggregate properties include the source of aggregates, size of aggregate, shape of aggregate, crushing type of aggregates, angularity index, surface texture, modulus of elasticity, bulk density, specific gravity, absorption and moisture content, grading of aggregates. For a good concrete mix, aggregates need to be clean, hard, and strong with the particles free of absorbed chemicals or coatings of clay and other fine materials that are likely to interfere with the process of hydration.

2.2.1. Types of Aggregates

Aggregate characteristics have a significant effect on the behavior of fresh and hardened p rope r t i e s o f conc r e t e . Ag g r eg a t e

characteristics are function of particle size and as such, the following classification is used in accordance to common practice: material retained in the No.4 sieve (4.75mm) is considered as coarse aggregate; material passing No.4 sieve (4.75mm) and retained in the No. 200 sieve (75μm) is considered as fine aggregate; and material passing No. 200 sieve is referred to as micro-fines.

2.2.2. Properties of Aggregates

The main characteristics of aggregate that affect the performance of fresh and hardened concrete, even though some variation in aggregate properties is expected, are as follows:

2.2.3. Shape and Texture The shape and texture of both coarse and fine aggregates play a significant role in the properties fresh and hardened concrete. The shape and texture of coarse aggregate play an important role on the behavior of fresh and hardened concrete as they affect the demand for fine aggregate.

Flaky and elongated particles should be limited to between 35 to 40 percent, or the shape coefficient determined by Equation 3.1 which should not be less than 0.20.

where is the volume of particle I

is the size of particle I

High voids, Poor Bond Grip, Bleeding.

Good Bond Grip

Increase segregation, Finishing

Elongated

Rough

Water Demand.

Table 3: Impact of aggregates shape and texture in concrete.

Properties

Influence on Concrete Performance

Bonding, Water Demand, Absorption

Cohension, Water Demand (Strength)

Table 2: Aggregate properties and its influence on concrete performance.

Strength, Water demand

CONCRETE MIX DESIGN MANUAL

2.2.4. Maximum Size of Aggregate Maximum size of aggregate, MSA, influences workabil ity, strength, shrinkage, and permeability. Mixtures with large maximum size of coarse aggregate tend to produce concrete with better workability, probably because of the decrease in specific surface. There is an optimal maximum size of coarse aggregate that produces the highest strength for a given consistency and cement content. In high- performance concrete (HPC) with low water- cement ratio and high cement content, a high value of MSA tends to reduce strength. This can be explained by the observation that bond with large particles tends to be weaker than with small particles due to smaller surface area-to- volume ratios. Mixtures with coarse aggregates having large maximum size tends to have reduced shrinkage and creep. Finally, for a given water-cement ratio, the permeability increases as the maximum size of the aggregate increases.

2.2.5. Limit on Deleterious Matter. In natural sands, deleterious particles like clay minerals and organic matter, mostly present in the minus 63μm portion, increase significantly the demand for water. It is recommended that the limit of 5% passing 63μm be adopted for use in concrete mix design.

2.2.6. Aggregates in Nigerian Construc- tion Industry The aggregates commonly available in the Nigerian construction industry are the fine aggregates [sharp sand and stone dust] and coarse aggregates [natural gravel and crushed rock]. In selecting aggregates for use in concrete, the grading curve for such an

aggregate is an important parameter for determining its suitability for use.

EN 12620 Aggregate for Concrete provides

grading limits within which suitable aggregates

are expected to lie.

The maximum size of coarse aggregate is the

standard sieve size through which at least 90%

of the coarse aggregates would pass. Typical

maximum sizes of aggregate in use in Nigeria

are 40mm, 20mm and 10mm with 20mm being

the most common. The maximum size of

aggregate affects the workability and strength

of the concrete. It also affects the required

water content for a certain workability and fine

aggregate content required for achieving a

cohesive mix.

1 2

.......... 3.1

[ ....... ] 6

n

n

1 2 3 4 5 6

LOWER LIMIT FOR 20MM 10 - 15MM AGGREGATE

LOWER LIMIT FOR 20MM 5-15MM AGGREGATE UPPER LIMIT FOR 20MM

100

90

80

70

60

50

40

30

20

10

0

Fig. 2 - Grading curve for 5-15 coarse aggregate

SIEVE NO

CONCRETE MIX DESIGN MANUAL

2.2.4. Maximum Size of Aggregate Maximum size of aggregate, MSA, influences workabil ity, strength, shrinkage, and permeability. Mixtures with large maximum size of coarse aggregate tend to produce concrete with better workability, probably because of the decrease in specific surface. There is an optimal maximum size of coarse aggregate that produces the highest strength for a given consistency and cement content. In high- performance concrete (HPC) with low water- cement ratio and high cement content, a high value of MSA tends to reduce strength. This can be explained by the observation that bond with large particles tends to be weaker than with small particles due to smaller surface area-to- volume ratios. Mixtures with coarse aggregates having large maximum size tends to have reduced shrinkage and creep. Finally, for a given water-cement ratio, the permeability increases as the maximum size of the aggregate increases.

2.2.5. Limit on Deleterious Matter. In natural sands, deleterious particles like clay minerals and organic matter, mostly present in the minus 63μm portion, increase significantly the demand for water. It is recommended that the limit of 5% passing 63μm be adopted for use in concrete mix design.

2.2.6. Aggregates in Nigerian Construc- tion Industry The aggregates commonly available in the Nigerian construction industry are the fine aggregates [sharp sand and stone dust] and coarse aggregates [natural gravel and crushed rock]. In selecting aggregates for use in concrete, the grading curve for such an

aggregate is an important parameter for determining its suitability for use.

EN 12620 Aggregate for Concrete provides

grading limits within which suitable aggregates

are expected to lie.

The maximum size of coarse aggregate is the

standard sieve size through which at least 90%

of the coarse aggregates would pass. Typical

maximum sizes of aggregate in use in Nigeria

are 40mm, 20mm and 10mm with 20mm being

the most common. The maximum size of

aggregate affects the workability and strength

of the concrete. It also affects the required

water content for a certain workability and fine

aggregate content required for achieving a

cohesive mix.

1 2

.......... 3.1

[ ....... ] 6

n

n

1 2 3 4 5 6

LOWER LIMIT FOR 20MM 10 - 15MM AGGREGATE

LOWER LIMIT FOR 20MM 5-15MM AGGREGATE UPPER LIMIT FOR 20MM

100

90

80

70

60

50

40

30

20

10

0

Fig. 2 - Grading curve for 5-15 coarse aggregate

SIEVE NO

7

The larger the size of the maximum aggregate, the lower the surface area of the coarse aggregates. With a higher surface area, a higher water content is required to coat the particles and develop workability. Also, a higher maximum size of aggregate would require a lower fine aggregate content to coat the particles and maintain cohesiveness of the concrete mix. This implies that for the same workability, coarse aggregate with maximum size of 40mm would require a lower water cement ratio and thus higher strength compared to coarse aggregate with maximum size of 20mm. However, maximum size of aggregate is restricted by the clear cover and the minimum distance between reinforcement bars. See EN 12620 Aggregates for Concrete.

2.2.8. Grading and Type of Aggregate

Typically, aggregates can be single sized or graded in terms of particle size distribution. The grading of aggregate is significant in achieving a dense and cohesive concrete mix. The voids created by the larger coarse aggregates are filled by the smaller coarse aggregates and hence, the volume of cement-sand-water paste required to fill the final voids is minimum. By proper grading of coarse aggregate, the compactibility of concrete is improved and segregation is minimized especially for higher workability.

The type and source of aggregate also has a

significant effect on the compressive strength

of concrete. Typical aggregates in use in Nigeria

can be categorized in the crushed and

uncrushed classes. It is widely accepted that

concrete produced from crushed aggregate has

a higher strength compared to concrete

produced from uncrushed aggregates. This can

be attributed to the rough surface texture of the

crushed aggregates which gives it a better

bonding with the cement gel. The grading of

aggregate is significant in attaining an

economical mix as it affects the amount of concrete that can be obtained with a given amount of cement and water.

2.3. ADMIXTURES Admixtures are constituent materials other than Portland cement, aggregate and water added to concrete mixture before or during mixing to modify one or more characteristic of concrete either in the wet or hardened state. Admixtures can be group into two major group as Mineral admixtures and Chemical Admixtures.

2.3.1. Mineral Admixtures Mineral admixtures are either naturally occurring or as by-product of industrial processes. They are known as supplementary cementing materials, which could be blended with clinker to produce blended or composite cement as specified in NIS 444-1 Mineral admixture could also be added during production of cement to alter characteristic performance of concrete.

2.3.1.1. Types of Mineral Admixtures

Ÿ Ground Granulated Blast Furnace Slag

Ÿ Fly Ash (Siliceous or Calcareous)

Ÿ Silica Fume

are the result of controlled calcination

of rice husk and kaolinite clay falls

under the calcined pozolana etc.

2.3.2. Chemical Admixtures

added to concrete to alter the characteristic

either at the wet or hardened state. The

composition and the performance criteria are

listed in EN 934-2 Admixtures for Concrete

Mortar and Grout.

CONCRETE MIX DESIGN MANUAL

The larger the size of the maximum aggregate, the lower the surface area of the coarse aggregates. With a higher surface area, a higher water content is required to coat the particles and develop workability. Also, a higher maximum size of aggregate would require a lower fine aggregate content to coat the particles and maintain cohesiveness of the concrete mix. This implies that for the same workability, coarse aggregate with maximum size of 40mm would require a lower water cement ratio and thus higher strength compared to coarse aggregate with maximum size of 20mm. However, maximum size of aggregate is restricted by the clear cover and the minimum distance between reinforcement bars. See EN 12620 Aggregates for Concrete.

2.2.8. Grading and Type of Aggregate

Typically, aggregates can be single sized or graded in terms of particle size distribution. The grading of aggregate is significant in achieving a dense and cohesive concrete mix. The voids created by the larger coarse aggregates are filled by the smaller coarse aggregates and hence, the volume of cement-sand-water paste required to fill the final voids is minimum. By proper grading of coarse aggregate, the compactibility of concrete is improved and segregation is minimized especially for higher workability.

The type and source of aggregate also has a

significant effect on the compressive strength

of concrete. Typical aggregates in use in Nigeria

can be categorized in the crushed and

uncrushed classes. It is widely accepted that

concrete produced from crushed aggregate has

a higher strength compared to concrete

produced from uncrushed aggregates. This can

be attributed to the rough surface texture of the

crushed aggregates which gives it a better

bonding with the cement gel. The grading of

aggregate is significant in attaining an

economical mix as it affects the amount of concrete that can be obtained with a given amount of cement and water.

2.3. ADMIXTURES Admixtures are constituent materials other than Portland cement, aggregate and water added to concrete mixture before or during mixing to modify one or more characteristic of concrete either in the wet or hardened state. Admixtures can be group into two major group as Mineral admixtures and Chemical Admixtures.

2.3.1. Mineral Admixtures Mineral admixtures are either naturally occurring or as by-product of industrial processes. They are known as supplementary cementing materials, which could be blended with clinker to produce blended or composite cement as specified in NIS 444-1 Mineral admixture could also be added during production of cement to alter characteristic performance of concrete.

2.3.1.1. Types of Mineral Admixtures

Ÿ Ground Granulated Blast Furnace Slag

Ÿ Fly Ash (Siliceous or Calcareous)

Ÿ Silica Fume

are the result of controlled calcination

of rice husk and kaolinite clay falls

under the calcined pozolana etc.

2.3.2. Chemical Admixtures

added to concrete to alter the characteristic

either at the wet or hardened state. The

composition and the performance criteria are

listed in EN 934-2 Admixtures for Concrete

Mortar and Grout.

CONCRETE MIX DESIGN MANUAL

2.3.2.1. T y p e s o f C h e m i c a l Admixtures Ÿ Water reducing/Plasticizing Ÿ High-range water reducing/super-

plasticizing Ÿ Water retaining (Reduces Bleeding) Ÿ Water resisting (for Waterproofing) Ÿ Air Entraining Ÿ Set Retarding Ÿ Set Accelerating Ÿ Hardening Accelerating

Others are; Ÿ Set retarding/water reducing/

plasticizing. Ÿ Set retarding/high-range water

reducing/super-plasticizing. Ÿ Set Accelerating/water reducing/

plasticizing.

Admixture could be used singularly or in combinations to attain any desired performance effect in concrete.

2.4. CONCRETE GRADES Concrete is generally designed in grades which, in Nigeria, correspond to classes of strength and therefore categories of concrete below those shown in the Table 5 should never be used. Consequently, the single most important deleterious effect on building strength and durability is poor concreting. The concrete should be 'designed' OR 'designated'. In a 'designated concrete', the producer who is generally the constructor (not necessarily the same as a contractor) is required to produce a material to satisfy

the designated strength and consistency (workability) using a particular aggregate s ize. Designated concretes are designated as Grade 30, for example, based on the cube strength up to Grade 50, according to the application involved. A designed concrete, on the other hand, is the one whose strength class, cement type, and limits to composition including water/cement ratio, cement content (mix ratio) are specified.

The symbol f generally denotes ck

characteristic strength based on cylinder strength of the concrete. The term f denotes cube strength.cu

Prestressed & Reinforced concrete subject to chlorides

30C30/37 37

Minimum Characteristic

Cylinder Strength

Minimum Characteristic

Cube Strength

Table 4: Strength Classes of Concrete according to EN 206-1

9

Ÿ Water reducing/Plasticizing

Ÿ Air Entraining

Ÿ Set Retarding

Ÿ Set Accelerating

Ÿ Hardening Accelerating

Ÿ Set retarding/water reducing/ plasticizing.

Ÿ S e t r e t a rd i n g / h i g h - r a n g e wa t e r

reducing/super-plasticizing.

plasticizing.

combinations to attain any desired performance

effect in concrete.

2.4. CONCRETE GRADES

and therefore categories of concrete below

those shown in the Table 5 should never be

used. Consequently, the single most important

deleterious effect on building strength and

durability is poor concreting. The concrete

should be 'designed' OR 'designated'. In a

'designated concrete', the producer who is

generally the constructor (not necessarily the

same as a contractor) is required to produce a

material to satisfy the designated strength and

consistency (workability) using a particular

aggregate size. Designated concretes are

designated as Grade 30, for example, based on

the cube strength up to Grade 50, according to

the application involved. A designed concrete,

on the other hand, is the one whose strength

class, cement type, and limits to composition including water/cement ratio, cement content (mix ratio) are specified.

The symbol f genera l ly denotes c k

characteristic strength based on cylinder

strength of the concrete. The term f denotes cu

cube strength.

30C30/37 37

Minimum Characteristic

Cylinder Strength

Minimum Characteristic

Cube Strength

Table 4: Strength Classes of Concrete according to EN 206-1

9

CONCRETE MIX DESIGN MANUAL

3.1. Introduction to mix design For ease of calculation, the mix design procedure is divided into five stages. Each step by step procedure deals with a particular aspect and ends with an important parameter. The step by step procedure is as follows:

Step 1: Determination of target mean strength Step 2: Determination of Water-cement ratio Step 3: Determination of water content Step4: Determination of cement content Step5: Determination of aggregate content

3.2. Determination of Target Mean Strength

As a result of the variability of concrete in production, it is necessary to design the mix to have a mean strength greater than the specified characteristic strength. Hence, the target compressive strength is obtained from the equation:

where f = the target mean strengthm

f = the specified characteristic c strength k = a constant (taken as 1.64 for a 5% defective level) s = standard deviation

Typically, the standard deviation is obtained from the field by carrying out tests on a minimum of 20-30 samples taken from the site as early as possible. In cases of significant changes in production of concrete batches, the standard deviation value should be calculated for new batches. The standard deviation recommended in this manual is 6MPa. Where however a producer is able to achieve lesser value, he can use his own value.

3.3. Determination of Water- Cement ratio

Different cements and aggregates of various maximum size, grading and other characteristics may produce concretes of different compressive strengths at the same water-cement ratio. Hence, the relationship between strength and water cement ratio should be established for the materials to be used. If this is not available, the free water-cement ratio corresponding to the target strength may be obtained from Fig. 4.1 The water cement ratio selected should be checked against the maximum water cement ratio for the requirements of durability and the lower of the two values is recommended.

PART THREE: MIX DESIGN PROCEDURE

10

For ease of calculation, the mix design

procedure is divided into five stages. Each step

by step procedure deals with a particular aspect

and ends with an important parameter. The

step by step procedure is as follows:

Step 1: Determination of target mean strength

Step 2: Determination of Water-cement ratio

Step 3: Determination of water content

Step4: Determination of cement content

Step5: Determination of aggregate content

3.2. Determination of Target Mean

Strength

have a mean strength greater than the specified

characteristic strength. Hence, the target

compressive strength is obtained from the

equation:

where f = the target mean strengthm

f = the specified characteristic c strength k = a constant (taken as 1.64 for a 5% defective level) s = standard deviation

Typically, the standard deviation is obtained from the field by carrying out tests on a minimum of 20-30 samples taken from the site as early as possible. In cases of significant changes in production of concrete batches, the standard deviation value should be calculated for new batches. The standard deviation recommended in this manual is 6MPa. Where however a producer is able to achieve lesser value, he can use his own value.

3.3. Determination of Water-Cement ratio

Different cements and aggregates of various max imum s i ze , g rad ing and o ther characteristics may produce concretes of different compressive strengths at the same water-cement ratio. Hence, the relationship between strength and water cement ratio should be established for the materials to be used. If this is not available, the free water- cement ratio corresponding to the target strength may be obtained from Fig. 4.1 The water cement ratio selected should be checked against the maximum water cement ratio for the requirements of durability and the lower of the two values is recommended.

PART THREE: MIX DESIGN PROCEDURE

10

CONCRETE MIX DESIGN MANUAL

Alternatively, the equation of the strength versus water/cement graph for Grade 32.5 cement is for [ ]

Where is the target mean strength of the mix; r is the water/cement ratio From equation 4.1, we have:

The equation of the strength versus water/cement graph for Grade 42.5 cement is[for]:

Where is the target mean strength of the mix; r is the water/cement ratio From equation 4.3, we have:

It should be noted here that the procedure adopted limits the target mean strength for concrete using Grade 32.5 cement to 44MPa while that of Grade 42.5 cement is limited to 57MPa for water/cement ratios between 0.3 and 0.9.

It should be noted here that the procedure adopted limits the target mean strength for concrete using Grade 32.5 cement to 52MPa while that of Grade 42.5 cement is limited to 68MPa.

3.4. Determination of Water content The water content of concrete is dependent on the type and maximum size of concrete to give a specified workability. The ranges of slump covered in this manual are 30 to 60mm and 60 to 180mm. Maximum aggregate sizes are also limited to 20 and 40mm. The recommended water content are as shown on Table 4.1.

3.5. Determination of cement content The cement content is determined from the water-cement ratio and the quantity of water.

The resulting value should be checked against the maximum and minimum value specified If the specified maximum cement content is exceeded, a higher cement grade should be used to enable the producer meet this requirement. Alternatively, super plasticizers could be used to meet other requirement at the determined cement content. If the minimum cement content is higher that the earlier calculated value, this minimum value should be adopted and the water content should be recalculated to provide the same water/cement ratio at the specified minimum cement content.

3.6. Determination of aggregate content To determine the total aggregate content, an estimate of the density of the fully compacted concrete should be known. From tests carried out, a density value of 2400kg/m3 is recommended for use for all mixes using normal weight aggregates. The total aggregate is obtained from the relationship:

The fine and coarse aggregate content are

determined by obtaining the proportion of fine

aggregate in the total aggregate content. Due to

the fact that many coarse aggregates

Table 4. : Approximate Free water contents required to give various levels

of workability

6 4 6 2 . . . . . . . . . . [ 5 . 1 ]rs = - +

6 2 .. . .. . . .. . .[ 5 . 2 ]

8 3 .. . .. . . .. . .[ 5 . 4 ]

s- =

12

Alternatively, the equation of the strength versus water/cement graph for Grade 32.5 cement is for [ ]

Where is the target mean strength of the mix; r is the water/cement ratio From equation 4.1, we have:

The equation of the strength versus water/cement graph for Grade 42.5 cement is[for]:

Where is the target mean strength of the mix; r is the water/cement ratio From equation 4.3, we have:

It should be noted here that the procedure adopted limits the target mean strength for concrete using Grade 32.5 cement to 44MPa while that of Grade 42.5 cement is limited to 57MPa for water/cement ratios between 0.3 and 0.9.

It should be noted here that the procedure adopted limits the target mean strength for concrete using Grade 32.5 cement to 52MPa while that of Grade 42.5 cement is limited to 68MPa.

3.4. Determination of Water content The water content of concrete is dependent on the type and maximum size of concrete to give a specified workability. The ranges of slump covered in this manual are 30 to 60mm and 60 to 180mm. Maximum aggregate sizes are also limited to 20 and 40mm. The recommended water content are as shown on Table 4.1.

3.5. Determination of cement content The cement content is determined from the water-cement ratio and the quantity of water.

The resulting value should be checked against the maximum and minimum value specified If the specified maximum cement content is exceeded, a higher cement grade should be used to enable the producer meet this requirement. Alternatively, super plasticizers could be used to meet other requirement at the determined cement content. If the minimum cement content is higher that the earlier calculated value, this minimum value should be adopted and the water content should be recalculated to provide the same water/cement ratio at the specified minimum cement content.

3.6. Determination of aggregate content To determine the total aggregate content, an estimate of the density of the fully compacted concrete should be known. From tests carried out, a density value of 2400kg/m3 is recommended for use for all mixes using normal weight aggregates. The total aggregate is obtained from the relationship:

The fine and coarse aggregate content are

determined by obtaining the proportion of fine

aggregate in the total aggregate content. Due to

the fact that many coarse aggregates

Table 4. : Approximate Free water contents required to give various levels

of workability

6 4 6 2 . . . . . . . . . . [ 5 . 1 ]rs = - +

6 2 .. . .. . . .. . .[ 5 . 2 ]

8 3 .. . .. . . .. . .[ 5 . 4 ]

s- =

12

available from the quarries in Nigeria do not fit into the BS882 envelopes for coarse aggregates, the use of combined aggregate grading envelope is recommended. Two methods are recommended for determining the proportion of fine aggregates in the concrete.

The first involves plotting the grading curves of

the fine and coarse aggregates on the same axis

on the graph paper and determining the

percentage combinations of the two aggregates

which gives a grading very close to the median

of the BS882 envelope.

software developed by Professor Charles

Uko of the University of Uyo, Uyo, Nigeria

which automatically determines the most

suitable combination once values of

percentages passing different sieve sizes

are provided for the two aggregates.

The fine aggregate and coarse aggregate

contents are calculated from the relationships

3.7. Trial Mixes

checked using trial batches. The workability of

the first trial mix should be measured and if it's

different from the stipulated value, the water

content should be adjusted suitably. With the

adjusted water content, the mix design should

be recalculated with the original water-cement

ratio. Two more trial mixes should be made with

this adjusted water content but at varying water

cement ratios of ±10% of the original value.

The last three mixes provide sufficient

information on the relationship between

compressive strength and water-cement ratio.

This can be used to carry out mix proportions

for field trials using actual methods of concrete

production on site.

The issue of trial mix must be taken very seriously in view of the variables involved in

CONCRETE MIX DESIGN MANUAL

1 2 3 4 5 6 7 8 9 10

FINE SAND % PASSING 5-15 AGG% PASSING Bs882 ALL-IN MEAN

POINT A = 45%

POINT B =24%

G

Fig. 4.2 - Combined aggregate curves for fine sand and 5-15 coarse aggregate

POINT A = 45%

POINT B=17%

1 2 3 4 5 6 7 8 9 10

POINT A = 45%

POINT B =17%

Fig. 4.3 - Combined aggregate curves for fine sand and 10-15 coarse aggregate

Fig. 4.5 - Combined aggregate grading curve for 21% fines and 79% coarse SIEVE NO

1 2 3 4 5 6 7 8 9 10

LOWER LIMIT FOR 20MM UPPER LIMIT FOR 20MM COMB AGG [21:79]

[USING COMBAG 16]

G

100

90

80

70

60

50

40

30

20

10

0

100

90

80

70

60

50

40

30

20

10

0

Fig. 4.4 - Combined aggregate grading curve for 21% fines and 79% coarse

1 2 3 4 5 6 7 8 9 10

LOWER LIMIT FOR 20MM UPPER LIMIT FOR 20MM COMB AGG [21:79]

SIEVE NO

P E

R C

E N

TA G

E P

A S

S IN

G

13

available from the quarries in Nigeria do not fit into the BS882 envelopes for coarse aggregates, the use of combined aggregate grading envelope is recommended. Two methods are recommended for determining the proportion of fine aggregates in the concrete.

The first involves plotting the grading curves of

the fine and coarse aggregates on the same axis

on the graph paper and determining the

percentage combinations of the two aggregates

which gives a grading very close to the median

of the BS882 envelope.

software developed by Professor Charles

Uko of the University of Uyo, Uyo, Nigeria

which automatically determines the most

suitable combination once values of

percentages passing different sieve sizes

are provided for the two aggregates.

The fine aggregate and coarse aggregate

contents are calculated from the relationships

3.7. Trial Mixes

checked using trial batches. The workability of

the first trial mix should be measured and if it's

different from the stipulated value, the water

content should be adjusted suitably. With the

adjusted water content, the mix design should

be recalculated with the original water-cement

ratio. Two more trial mixes should be made with

this adjusted water content but at varying water

cement ratios of ±10% of the original value.

The last three mixes provide sufficient

information on the relationship between

compressive strength and water-cement ratio.

This can be used to carry out mix proportions

for field trials using actual methods of concrete

production on site.

The issue of trial mix must be taken very seriously in view of the variables involved in

POINT A = 45%

1 2 3 4 5 6 7 8 9 10

FINE SAND % PASSING 5-15 AGG% PASSING Bs882 ALL-IN MEAN

POINT A = 45%

POINT B =24%

G

Fig. 4.2 - Combined aggregate curves for fine sand and 5-15 coarse aggregate

100

90

80

70

60

50

40

30

20

10

0

1 2 3 4 5 6 7 8 9 10

POINT B =17%

Fig. 4.3 - Combined aggregate curves for fine sand and 10-15 coarse aggregate

Fig. 4.5 - Combined aggregate grading curve for 21% fines and 79% coarse SIEVE NO

1 2 3 4 5 6 7 8 9 10

LOWER LIMIT FOR 20MM UPPER LIMIT FOR 20MM COMB AGG [21:79]

[USING COMBAG 16]

G

100

90

80

70

60

50

40

30

20

10

0

100

90

80

70

60

50

40

30

20

10

0

Fig. 4.4 - Combined aggregate grading curve for 21% fines and 79% coarse

1 2 3 4 5 6 7 8 9 10

LOWER LIMIT FOR 20MM UPPER LIMIT FOR 20MM COMB AGG [21:79]

SIEVE NO

P E

R C

E N

TA G

E P

A S

S IN

concrete production.

WORKED EXAMPLES This example involves the design of a concrete mix using Grade 32.5 cement and river sand as fine aggregate. The coarse aggregate is 10-15mm crushed rock with sieve analysis already done and as shown on Fig.

15

the design of grade 30 concrete, using both

grade 32.5 cement and grade 42.5 cements

respectively. the coarse aggregate was crushed

rock with maximum aggregate size 20mm.

Fine aggregate was sharp sand and the

percentage fines used was determined after

sieve analysis and combination of aggregate

using the method recommended or the

software COMBA (see Fig. 5)

15

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

1

1.1

1.2

1.3

1.4

1.5

1.6

1.7

1.8

19

2

2.1

2.2

2.3

3

3.1

3.2

3.3

3.4

4

4.1

4.2

5

5.1

5.2

5.3

5.4

6

6.1

6.2

6.3

6.4

MIX DESIGN EXAMPLE FOR GRADE 30 CONCRETE [USING GRADE 32.5 CEMENT]

S/NO ITEM UNITS

20

225

NONE

30

4

6.56

36.56

32.5

0.40

Crushed

Uncrushed

STAGE 6 - Trial Mix Quantities Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

100mm cube 150mm cube

2.8 7.1 7.0 13.1

5.6 14.2 14.1 26.1

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

1

1.1

1.2

1.3

1.4

1.5

1.6

1.7

1.8

19

2

2.1

2.2

2.3

3

3.1

3.2

3.3

3.4

4

4.1

4.2

5

5.1

5.2

5.3

5.4

6

6.1

6.2

6.3

6.4

MIX DESIGN EXAMPLE FOR GRADE 30 CONCRETE [USING GRADE 32.5 CEMENT]

S/NO ITEM UNITS

20

235

NONE

30

4

6.56

36.56

32.5

0.40

Crushed

Uncrushed

STAGE 6 - Trial Mix Quantities Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

100mm cube 150mm cube

2.9 7.4 6.9 12.8

5.9 14.8 13.8 25.6

CONCRETE MIX DESIGN MANUAL

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

1

1.1

1.2

1.3

1.4

1.5

1.6

1.7

1.8

19

2

2.1

2.2

2.3

3

3.1

3.2

3.3

3.4

4

4.1

4.2

5

5.1

5.2

5.3

5.4

6

6.1

6.2

6.3

6.4

MIX DESIGN EXAMPLE FOR GRADE 30 CONCRETE [USING GRADE 42.5 CEMENT]

S/NO ITEM UNITS

20

225

NONE

30

4

6.56

36.56

42.5

0.55

Crushed

Uncrushed

STAGE 6 - Trial Mix Quantities Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

100mm cube 150mm cube

2.8 5.1 7.7 14.4

CONCRETE MIX DESIGN MANUAL

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

1

1.1

1.2

1.3

1.4

1.5

1.6

1.7

1.8

19

2

2.1

2.2

2.3

3

3.1

3.2

3.3

3.4

4

4.1

4.2

5

5.1

5.2

5.3

5.4

6

6.1

6.2

6.3

6.4

MIX DESIGN EXAMPLE FOR GRADE 30 CONCRETE [USING GRADE 42.5 CEMENT]

S/NO ITEM UNITS

20

235

NONE

30

4

6.56

36.56

42.5

0.55

Crushed

Uncrushed

STAGE 6 - Trial Mix Quantities Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

100mm cube 150mm cube

2.9 5.3 7.6 14.1

5.9 10.6 15.2 28.3

CONCRETE MIX DESIGN MANUAL

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

S/NO ITEM UNITS

Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

STAGE 6 - Trial Mix Quantities 100mm cube 150mm cube

18

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

S/NO ITEM UNITS

Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

STAGE 6 - Trial Mix Quantities 100mm cube 150mm cube

18

The following important points should

be noted when carrying out a mix design: 1. All cement brands to be used must be clearly labeled indicating the strength class 2. A site trial mix design should be carried out to ensure the suitability of the mix on site. Cubes should be cast during the trial and should be tested pr ior to the commencement of concreting works 3. Concrete mix design procedure assumes that aggregates are in the saturated surface dry condition. Hence, coarse aggregates should be wetted before use to bring them to this condition 4. Water cement ratio must be strictly controlled on the site as it governs the strength and workabil i ty of the concrete. 5. Ensure cement is stocked properly in a waterproof area and is not in direct contact with floor or walls 6. Cubes should always be cast for every batch of concrete. Ensure that a minimum o f t h r e e c u b e s a r e produced for 28days testing. 7. The following are essentials for a site laboratory:

· Set of 12 cube moulds of size

150mm

scale

25mm, 20mm, 12.5mm, 10mm,

and 4.75mm, 2.36mm, 1.18mm,

a pan and lid.

site, a suitable one should be identified

close to the site.

CONCRETE MIX DESIGN MANUAL

RECOMMENDATIONS The following important points should be noted when carrying out a mix design: 1. All cement brands to be used must be clearly labeled indicating the strength class 2. A site trial mix design should be carried out to ensure the suitability of the mix on site. Cubes should be cast during the trial and should be tested p r i o r t o t h e commencement of c o n c r e t i n g works 3. Concrete mix des ign procedure assumes that aggregates are in the saturated surface dry condition. Hence, coarse aggregates should be wetted before use to bring them to this condition 4. Water cement ratio must be strictly controlled on the site as it governs the s t r e n g t h a n d wo r k a b i l i t y o f t h e concrete. 5. Ensure cement is stocked properly in a waterproof area and is not in direct contact with floor or walls 6. Cubes should always be cast for every batch of concrete. Ensure that a minimum of three cubes are produced for 28days testing. 7. The following are essentials for a site laboratory:

· Set of 12 cube moulds of size

150mm

scale

25mm, 20mm, 12.5mm, 10mm,

and 4.75mm, 2.36mm, 1.18mm,

a pan and lid.

site, a suitable one should be identified close to

the site.

A.1. TESTING FRESH CONCR- ETE (SLUMP TEST) PROC- EDURE

A.1.1. Apparatus. · Slump cone · Base plate. · Compacting rod · Funnel · Ruler · Scoop · Timer · Shovel · Moist cloth

A.1.2. Testing Procedure · Mix or remix the concrete sample

thoroughly. · Dampen the inside of the slump cone,

the funnel and the base plate by wiping with a damp cloth.

· Clamp the slump cone to the base plate or stand firmly on the foot pieces to hold the slump down and in place.

· Fill the slump cone in 3 equal layer compacting each layer with 25 stroke of the tamping rod, distributing the strokes uniformly all over the surface of the layer. Repeat this for the second and the third layer tampering each layer through to the surface of the underlining layer.

· After compacting the third layer remove the funnel and strike off any excess concrete by means of sawing and the rolling motion of the tampering rod.

· Remove spilled concrete from the base plate and around the slump cone.

· Remove the slump cone by raising it vertically in a gentle manner within 5 to

10 seconds. · The operation from filling to the

remover of the slump cone should be done within 150 seconds.

· Immediately after the removal of the slump cone, measure and record the slump as the difference between the highest point on the concrete and the height of the slump cone to the nearest 10mm.

The result is valid only if the specimen yields a true slump. See EN 12350-2 Testing fresh concrete. Slump-test for more detail.

A . 2 . T E S T I N G H A R D E N E D CONCRETE (COMPRESSIVE TEST) PROCEDURE A.2.1. Sample Preparation

· Wipe the excess moisture on the test

specimen with a clean towel

· Wipe the surface of the platen on the

testing machine clean of any particle

especially from previous tests.

auxiliary platen or spacing blocks

between the specimen and the platens

of the testing machine.

so that the load is applied on the

smooth surfaces and not on the trowel

surface.

with the center of the upper and the

lower platen of the testing machine.

20

APPENDIX

A.1. TESTING FRESH CONCR- E T E ( S L U M P T E S T ) P R O C - EDURE

A.1.1. Apparatus. · Slump cone · Base plate. · Compacting rod · Funnel · Ruler · Scoop · Timer · Shovel · Moist cloth

A.1.2. Testing Procedure · Mix or remix the concrete sample

thoroughly. · Dampen the inside of the slump cone,

the funnel and the base plate by wip

FIRST EDITION: AUGUST 2017

SPECIAL PUBLICATION NO. COREN/2017/016/RC

CONCRETE MIX DESIGN MANUAL

ENGINEERING IN NIGERIA

ENGINEERING IN NIGERIA

1. Engr. Prof. Charles Uko, FNSE Chairman University of Uyo

2. Engr. K.A Ali, FNSE, NPOM, mni COREN

3. Engr. W. Kamila Maliki, FNSE, mni COREN

4. Engr. M.U. Adoyi, FNSE COREN

5. Engr. A. J. Agabi, MNSE COREN

6. Engr. Lukman Sani, MNSE COREN

7. Engr. Ahmed A.S.Y. Kutigi, MNSE COREN

8. Engr. Prof. Danladi S. Matawal, MNSE NBBRI

9. Engr. (Mrs. Emeso B. Ojo, MNSE NBBRI

10. Engr. Gai F. Iliya, MNSE NBBRI

11. Mr. George Omange NBBRI

12. Engr. Bukola S. Adebisi, MNSE LAFARGE

13. Dr. Abdullahi S.B. Gimba LAFARGE

14. Mr. Vipul Agrawal LAFARGE

15. Engr. Femi Yusuf, MNSE LAFARGE

16. Engr. M.I. Nwoye, FNSE JULIUS BERGER

17. Engr. Joern Seitz JULIUS BERGER

18. Engr. Mustapha Olu JULIUS BERGER

19. Mr. M. Jagdish DANGOTE

20. Engr. Ben Ani NSE

ii

S/N NAME/ INTEREST INSTITUTION

1. Engr. Prof. Charles Uko, MNSE Chairman Council for the Regulation of Engineering in Nigeria.

2. Engr. Kashim A. Ali, FNSE, NPOM, mni Council for the Regulation of Engineering in Nigeria.

3. Engr. Kamila W. Maliki, FNSE, mni Council for the Regulation of Engineering in Nigeria.

4. Engr. M.U. Adoyi, FNSE Council for the Regulation of Engineering in Nigeria.

5. Engr. A. J. Agabi, MNSE Council for the Regulation of Engineering in Nigeria.

6. Engr. Lukman Sani, MNSE Council for the Regulation of Engineering in Nigeria.

7. Engr. Ahmed A.S.Y. Kutigi, MNSE Council for the Regulation of Engineering in Nigeria.

8. Engr. Prof. Danladi S. Matawal, MNSE Nigeria Building and Road Research Institute.

9. Engr. (Mrs.) Emeso B. Ojo, MNSE Nigeria Building and Road Research Institute.

10. Engr. Gai F. Iliya, MNSE Nigeria Building and Road Research Institute.

11. Mr. George Omange Nigeria Building and Road Research Institute.

12. Engr. Ben Ani Nigerian Society of Engineers.

13. Engr. M.I. Nwoye, FNSE Julius Berger Nigeria Plc.

14. Engr. Joern Seitz Julius Berger Nigeria Plc.

15. Engr. Mustapha Olu Julius Berger Nigeria Plc.

16. Mr. M. Jagdish Dangote Cement Plc.

17. Engr. Bukola S. Adebisi, MNSE Lafarge Africa Plc.

18. Mr. Vipul Agrawal Lafarge Africa Plc.

19. Engr. Femi Yusuf, MNSE Lafarge Africa Plc.

iii

FOREWORD

It is with deep sense of joy that the Council for the Regulation of Engineering in Nigeria, COREN, present the Concrete Mix Design Manual for Nigeria. This is indeed historic, as sad as it is, we must admit that this is the first of its type as the nation had never had her own Concrete Mix Design Manual. Like in many areas of our national life, we had all these years depended on the Concrete Mix Design Manual of other nations irrespective of their sharp differences in their environmental and other factors.

The challenge was heightened when in 2014, controversies became pervasive as to classes and qualities of cement. Eventhough the issues on the subject were promptly put to rest with the conclusion that cement classification does not cause building collapse but rather its application.

This, and the need to take up a national industry challenge, compelled COREN to commence the project of producing the Concrete Mix Design Manual for Nigeria.

The journey has been chequered with various challenges all of which were proficiently surmounted in the course of the project.

It started with the formation of a Technical Committee with membership carefully selected from the academia and the industry. The work of the Committee included laboratory tests, the results of which were variously subjected to further confirmation tests carried out in various Universities in the geo-political zones of Nigeria. The work was further subjected to critique analysis to arrive at a document that has no doubt, met international standard and the test of time.

The Concrete Mix Design Manual for Nigeria, like any document of this nature must be subjected to periodic review. Every reference document goes obsolete if left to drift for eternity, that is, without review.

The Manual, for practitioners in Nigeria using concrete, must now replace the foreign manuals which has produced the danger of non-uniformity because of diverse sources. The Concrete Mix Design Manual for Nigeria, therefore, provides homogeneity for all concrete design.

In the application of this manual, a trial mix is mandatory for any major construction site in Nigeria.

On behalf of the COREN, I wish to express my profound appreciation to the Chairman and members of the Technical Committee, the various construction companies which readily gave their support to this project, the Universities which made their laboratories and personnel available, the Management and staff of the Nigerian Building and Road Research Institute, NBRRI, Lafarge Cement, Dangote Cement and those of COREN who committed so much of their time and energy to this project.

This is indeed a historic achievement but opening the window of challenges in our need to develop our indigenous Codes and standards as we take Engineering Practice to higher levels in Nigeria.

Engr. Kashim A. Ali, FNSE, mni

President, COREN

iii

FOREWORD

It is with deep sense of joy that the Council for the Regulation of Engineering in Nigeria, COREN, present the Concrete Mix Design Manual for Nigeria. This is indeed historic, as sad as it is, we must admit that this is the first of its type as the nation had never had her own Concrete Mix Design Manual. Like in many areas of our national life, we had all these years depended on the Concrete Mix Design Manual of other nations irrespective of their sharp differences in their environmental and other factors.

The challenge was heightened when in 2014, controversies became pervasive as to classes and qualities of cement. Eventhough the issues on the subject were promptly put to rest with the conclusion that cement classification does not cause building collapse but rather its application.

This, and the need to take up a national industry challenge, compelled COREN to commence the project of producing the Concrete Mix Design Manual for Nigeria.

The journey has been chequered with various challenges all of which were proficiently surmounted in the course of the project.

It started with the formation of a Technical Committee with membership carefully selected from the academia and the industry. The work of the Committee included laboratory tests, the results of which were variously subjected to further confirmation tests carried out in various Universities in the geo-political zones of Nigeria. The work was further subjected to critique analysis to arrive at a document that has no doubt, met international standard and the test of time.

The Concrete Mix Design Manual for Nigeria, like any document of this nature must be subjected to periodic review. Every reference document goes obsolete if left to drift for eternity, that is, without review.

The Manual, for practitioners in Nigeria using concrete, must now replace the foreign manuals which has produced the danger of non-uniformity because of diverse sources. The Concrete Mix Design Manual for Nigeria, therefore, provides homogeneity for all concrete design.

In the application of this manual, a trial mix is mandatory for any major construction site in Nigeria.

On behalf of the COREN, I wish to express my profound appreciation to the Chairman and members of the Technical Committee, the various construction companies which readily gave their support to this project, the Universities (especially the University of Uyo, Uyo) which made their laboratories and personnel available, the Management and staff of the Nigerian Building and Road Research Institute, NBRRI, Lafarge Cement, Dangote Cement and those of COREN who committed so much of their time and energy to this project.

This is indeed a historic achievement but opening the window of challenges in our need to develop our indigenous Codes and standards as we take Engineering Practice to higher levels in Nigeria.

Engr. Kashim A. Ali, FNSE, mni

President, COREN August, 2017

Council for the Regulation of Engineering in Nigeria i

Technical Team ii

1.3. Requirements of Concrete Mix Design 1

1.4. Variability of Concrete Strength 2 - 3

1.5. Selecting Mix Characteristics 3

1.6. Decision Variables in Mix Design 3

1.6.1 Water Cement ratio 3

1.6.2 Cement Content 3

1.7.1 Compressive Strength 4

2.2. AGREGATES 6

2.2.3 Shape and Texture 6 - 7

PART TWO: NIGERIAN CEMENT, AGGREGATE, ADMIXTURE AND

CONCRETE STANDARDS

Council for the Regulation of Engineering in Nigeria i

Technical Team ii

1.3. Requirements of Concrete Mix Design 1

1.4. Variability of Concrete Strength 2 - 3

1.5. Selecting Mix Characteristics 3

1.6. Decision Variables in Mix Design 3

1.6.1 Water Cement ratio 3

1.6.2 Cement Content 3

1.7.1 Compressive Strength 4

2.2. AGREGATES 6

2.2.3 Shape and Texture 6 - 7

PART TWO: NIGERIAN CEMENT, AGGREGATE, ADMIXTURE AND

CONCRETE STANDARDS

2.2.7 Maximum Nominal Size of Aggregate 7 - 8

2.2.8 Grading and Type of Aggregate 8

2.3. ADMIXTURES 8

2.3.2. Chemical Admixtures 8

2.4. CONCRETE GRADES 9

3.1. Introduction to mix design 10

3.2. Determination of Target Mean Strength 10

3.3. Determination of Water-Cement ratio 10 - 11

3.4. Determination of Water content 12

3.5. Determination of cement content 12

3.6. Determination of aggregate content 12 - 13 3.7. Trial Mixes 13 - 15

v

2.2.7 Maximum Nominal Size of Aggregate 7 - 8

2.2.8 Grading and Type of Aggregate 8

2.3. ADMIXTURES 8

2.3.2. Chemical Admixtures 8

2.4. CONCRETE GRADES 9

3.1. Introduction to mix design 10

3.2. Determination of Target Mean Strength 10

3.3. Determination of Water-Cement ratio 10 - 11

3.4. Determination of Water content 12

3.5. Determination of cement content 12

3.6. Determination of aggregate content 12 - 13 3.7. Trial Mixes 13 - 15

3.8. Worked examples 15 - 18

v

LIST OF TABLES

Table1: Strength ranges for various grades of cement in use in Nigeria.

Table 2: Aggregate properties and its influence on concrete performance.

Table 3: Impact of aggregates shape and texture in concrete.

Table 4: Strength Classes of Concrete according to EN 206-1

Table 5: Approximate Free water contents required to give various levels of workability

LIST OF FIGURES

Fig 2 Grading Curve for 5-15 Coarse Aggregate

Fig 3 Strength versus water/cement Ratio for Nigeria Cements

Fig 4.1 Combined aggregate curves for curves for fine sand and 5-15 coarse

aggregate.

Fig 4.2 Combined aggregate curves for curves for fine sand and 10-15 coarse

aggregate.

Fig 4.3 Combined aggregate grading curve for 21% fine and 79% coarse

Fig 4.4 Combined aggregate grading curve for 21% fines and 79% coarse using

COMBAG16

vi

LIST OF TABLES

Table1: Strength ranges for various grades of cement in use in Nigeria.

Table 2: Aggregate properties and its influence on concrete performance.

Table 3: Impact of aggregates shape and texture in concrete.

Table 4: Strength Classes of Concrete according to EN 206-1

Table 5: Approximate Free water contents required to give various levels of workability

LIST OF FIGURES

Fig 2 Grading Curve for 5-15 Coarse Aggregate

Fig 3 Strength versus water/cement Ratio for Nigeria Cements

Fig 4.1 Combined aggregate curves for curves for fine sand and 5-15 coarse

aggregate.

Fig 4.2 Combined aggregate curves for curves for fine sand and 10-15 coarse

aggregate.

Fig 4.3 Combined aggregate grading curve for 21% fine and 79% coarse

Fig 4.4 Combined aggregate grading curve for 21% fines and 79% coarse using

COMBAG16

vi

CONCRETE MIX DESIGN MANUAL

1.1. Scope This manual provides guidelines for the determination of the appropriate concrete mixes required for various construction applications. It provides a step by step procedure required for deducing the appropriate quantities of constituents required to achieve concrete with specified characteristics in accordance to EN 206. This manual is applicable for designing concrete mixes using Portland Limestone Cements conforming to NIS 444-1 and natural aggregates in conformity to EN 12620. With the advent of various strength classes of cement for construction, it is now possible to use any strength class of cement to obtain concrete of a specified characteristic strength provided the mix design is carried out appropriately. This mix design manual sets out the guidelines for concrete mixes in Nigeria.

1.2. Concept of Mix Design Concrete can be designed for strength ranging from 10MPa to 100MPa(note that

2 MPa is used instead of N/mm throughout this manual)making it an extremely versatile building material. In all these cases, the basic constituents remain the same, but it is their relative proportions that determine the properties.

In designing a concrete mix, the primary objective is to select suitable constituent materials and determine their required amounts in order to produce concrete of specific characteristics and properties as economically as possible. The characteristics typically specified are workability, strength and durability. Other characteristics that may be required includes; density, thermal characteristics, elastic modulus etc.

However, the mix design process only considers the factors which have a major effect on the properties of concrete i.e. workability, strength and durability. The proportioning of the constituent materials of concrete is dependent on the required performance of concrete in two states: the fresh/plastic and hardened states. Four variable factors need to be considered in mix proportioning:

i. Water-cement ratio ii. Cement content iii. Gradation of aggregates iv. Consistency

Typically, two or three factors are specified and the others are adjusted to achieve minimum workability and economy. In summary, the goal of mix proportioning is to use the minimum quantity of cement that will lubricate the mixture when fresh to allow for adequate placing and at the same time, bind the aggregates together and fill up the voids between them when the concrete has hardened. Any excess of paste results in a higher cost, higher drying shrinkage.

1.3. Requirements of Concrete Mix Design At the mix design stage, available data for deriving the required proportions of constituent materials is usually limited. The data provided in this manual are estimates and should be replaced where there is more appropriate data with regards to the local materials.

Part one: Introduction to Concrete Mix Design

1

CONCRETE MIX DESIGN MANUAL

1.1. Scope This manual provides guidelines for the determination of the appropriate concrete mixes required for various construction applications. It provides a step by step procedure required for deducing the appropriate quantities of constituents required to ach ieve concre te wi th spec i f i ed characteristics in accordance to EN 206. This manual is applicable for designing concrete mixes using Portland Limestone Cements conforming to NIS 444-1 and natural aggregates in conformity to EN 12620. With the advent of various strength classes of cement for construction, it is now possible to use any strength class of cement to obtain concrete of a specified characteristic strength provided the mix design is carried out appropriately. This mix design manual sets out the guidelines for concrete mixes in Nigeria.

1.2. Concept of Mix Design Concrete can be designed for strength ranging from 10MPa to 100MPa(note that MPa is used

2instead of N/mm throughout th is manual)making it an extremely versatile building material. In all these cases, the basic constituents remain the same, but it is their relative proportions that determine the properties.

In designing a concrete mix, the primary objective is to select suitable constituent materials and determine their required amounts in order to produce concrete of specific characteristics and properties as economically as possible. The characteristics typically specified are workability, strength and durability. Other characteristics that may be required includes; density, thermal characteristics, elastic modulus etc.

However, the mix design process only considers the factors which have a major effect on the properties of concrete i.e. workability, strength and durability. The proportioning of the

constituent materials of concrete is dependent on the required performance of concrete in two states: the fresh/plastic and hardened states. Four variable factors need to be considered in mix proportioning:

i. Water-cement ratio ii. Cement content iii. Gradation of aggregates iv. Consistency

Typically, two or three factors are specified and the others are adjusted to achieve minimum workability and economy. In summary, the goal of mix proportioning is to use the minimum quantity of cement that will lubricate the mixture when fresh to allow for adequate placing and at the same time, bind the aggregates together and fill up the voids between them when the concrete has hardened. Any excess of paste results in a higher cost, higher drying shrinkage.

1.3. Requirements of Concrete Mix Design At the mix design stage, available data for deriving the required proportions of constituent materials is usually limited. The data provided in this manual are estimates and should be replaced where there is more appropriate data with regards to the local materials.

Part one: Introduction to Concrete Mix Design

1

Mean Strength

The necessary data required can be classified

into two categories viz a viz: a. Specified variables: These are variables which are normally selected in the specifications based on intended use of the concrete. They include:

· The minimum compressive strength

concrete

available compaction equipment

· Maximum water-cement ratio

· Maximum/minimum cement content

· Strength class of cement

· Maximum aggregate size

b. Additional information: This refers to data on the available materials required for the concrete mix. They include: · The standard deviation which is a measure of the variability from the specified characteristic strength · The type of aggregate · Specific gravity of aggregate · Grading of fine aggregate

Understanding the basic concept of mix design is as significant as the actual calculations required for determining the mix proportions. In fact, the appropriate mix proportions are a consequence of the concrete mix design.

1.4. Variability of Concrete Strength In the production of concrete, there are inevitable variations in the properties of the

materials used as well as the construction methods. For instance, the quality of various batches of cement supplied may vary, or the grading and particle shape of the aggregates may vary. These variations may even be observed within a batch as a result of process of sampling, production, curing and testing of specimens even if they are conducted in accordance with the recommended standard. This results in variation of strength from batch to batch and also within a batch. This makes the strength of the final product difficult to assess.

In concrete mix design, it is now generally accepted that the variation in concrete strengths follow the normal distribution curve shown in Figure 1.1. The area under the curve represents the total number of test results. If a vertical line is drawn through a specified value, the proportion of results less than that value is represented by the area beneath the curve and to the left hand side of the vertical line as demonstrated in Figure 1.1. The normal distribution curve is defined by two parameters: its mean and standard deviation. The curve is symmetrical about its mean and the standard deviation is a measure of the variability. Typically at a given level of quality control, the standard deviation increases as the specified characteristic strength.

2

Mean Strength

The necessary data required can be classified

into two categories viz a viz: a. Specified variables: These are variables which are normally selected in the specifications based on intended use of the concrete. They include:

· The minimum compressive strength

concrete

available compaction equipment

· Maximum water-cement ratio

· Maximum/minimum cement content

· Strength class of cement

· Maximum aggregate size

b. Additional information: This refers to data on the available materials required for the concrete mix. They include: · The standard deviation which is a measure of the variability from the specified characteristic strength · The type of aggregate · Specific gravity of aggregate · Grading of fine aggregate

Understanding the basic concept of mix design is as significant as the actual calculations required for determining the mix proportions. In fact, the appropriate mix proportions are a consequence of the concrete mix design.

1.4. Variability of Concrete Strength In the production of concrete, there are inevitable variations in the properties of the

materials used as well as the construction methods. For instance, the quality of various batches of cement supplied may vary, or the grading and particle shape of the aggregates may vary. These variations may even be observed within a batch as a result of process of sampling, production, curing and testing of specimens even if they are conducted in accordance with the recommended standard. This results in variation of strength from batch to batch and also within a batch. This makes the strength of the final product difficult to assess.

In concrete mix design, it is now generally accepted that the variation in concrete strengths follow the normal distribution curve shown in Figure 1.1. The area under the curve represents the total number of test results. If a vertical line is drawn through a specified value, the proportion of results less than that value is represented by the area beneath the curve and to the left hand side of the vertical line as demonstrated in Figure 1.1. The normal distribution curve is defined by two parameters: its mean and standard deviation. The curve is symmetrical about its mean and the standard deviation is a measure of the variability. Typically at a given level of quality control, the standard deviation increases as the specified characteristic strength.

2

CONCRETE MIX DESIGN MANUAL

This statistical quality control method prov ides a sc ient i f i c approach to understanding the variations that are encountered on site so as to provide proper tolerance to allow for inevitable variations. To obtain the standard deviation on site, the minimum number of test samples should be between 20 to 30. The standard deviation used for any calculation should be based on either result obtained from the site, or in the absence of such data, assumed values are specified in different standards. Most producers of concrete in Nigeria do not have the quality control ability to have small standard deviations. To this end it is suggested that producers without adequate records start with a standard deviation of 6MPa, if thereafter a consecutive result of 30 tests is available, the standard deviation should be based on the result from the 30 consecutive tests. Whenever the producer is convinced that he can achieve a lower standard deviation, he can use that new value for mix design. 1.5. Selecting Mix Characteristics

The primary objective of the mix design is to

achieve the specified properties in the most

economical manner.

materials and mixture characteristics can the

specified properties be obtained in concrete

construction. As a result, adequate knowledge

of the constituent material properties and

properties of concrete in the plastic condition

is a prerequisite for a proper mix design. Also,

the exposure conditions and the intended use

of the concrete are also factored in whilst

carrying out the mix design as the

characteristics of the concrete should reflect

the needs of the structure.

Once the required characteristics have been

selected, the mixture is proportioned using data obtained from the field or the laboratory to achieve the specified requirements.

1.6. Decision Variables in Mix Design

The following are the key decision variables

when estimating the proportions in a concrete

mix:

important parameter that determines the

strength and durability of concrete. The

strength of concrete is dependent on the

water cement ratio and not totally on the

cement content. According to Abram's law,

the higher the water cement ratio, the lower

the strength of concrete. It is generally

accepted as a rule of thumb that every 1%

increase in quantity of water added reduces

the strength of concrete by 5%. Theoretically,

a water cement ratio of 0.25 is required for the

complete hydration of cement. Hence, it is

very important to control the water cement

ratio on site.

1.6.2. Cement Content Cement is the binder material in concrete which imparts strength to the concrete. With regards to durability, conditions of exposure govern the maximum cement contents required. For a given workability, a certain water content is required. This implies that a higher cement content would be required to achieve a desired workability at a lower water cement ratio. Based on the relationship between cement content and water cement ratio, we see that a greater water cement ratio would require a lower cement content. Details

3

CONCRETE MIX DESIGN MANUAL

This statistical quality control method provides a scientific approach to understanding the variations that are encountered on site so as to provide proper tolerance to allow for inevitable variations. To obtain the standard deviation on site, the minimum number of test samples should be between 20 to 30. The standard deviation used for any calculation should be based on either result obtained from the site, or in the absence of such data, assumed values are specified in different standards. Most producers of concrete in Nigeria do not have the quality control ability to have small standard deviations. To this end it is suggested that producers without adequate records start with a standard deviation of 6MPa, if thereafter a consecutive result of 30 tests is available, the standard deviation should be based on the result from the 30 consecutive tests. Whenever the producer is convinced that he can achieve a lower standard deviation, he can use that new value for mix design. 1.5. Selecting Mix Characteristics

The primary objective of the mix design is to

achieve the specified properties in the most

economical manner.

materials and mixture characteristics can the

specified properties be obtained in concrete

construction. As a result, adequate knowledge

of the constituent material properties and

properties of concrete in the plastic condition is

a prerequisite for a proper mix design. Also, the

exposure conditions and the intended use of the

concrete are also factored in whilst carrying out

the mix design as the characteristics of the

concrete should reflect the needs of the

structure.

Once the required characteristics have been

selected, the mixture is proportioned using data obtained from the field or the laboratory to achieve the specified requirements.

1.6. Decision Variables in Mix Design

The following are the key decision variables

when estimating the proportions in a concrete

mix:

important parameter that determines the

strength and durability of concrete. The

strength of concrete is dependent on the water

cement ratio and not totally on the cement

content. According to Abram's law, the higher

the water cement ratio, the lower the strength of

concrete. It is generally accepted as a rule of

thumb that every 1% increase in quantity of

water added reduces the strength of concrete by

5%. Theoretically, a water cement ratio of 0.25 is

required for the complete hydration of cement.

Hence, it is very important to control the water

cement ratio on site.

1.6.2. Cement Content Cement is the binder material in concrete which imparts strength to the concrete. With regards to durability, conditions of exposure govern the maximum cement contents required. For a given workability, a certain water content is required. This implies that a higher cement content would be required to achieve a desired workability at a lower water cement ratio. Based on the relationship between cement content and water cement ratio, we see that a greater water cement ratio would require a lower cement content. Details on properties and types of cement and how they relate to concrete properties are presented in chapter two of this manual.

1.6.3. Relative Proportion of Aggregates

Aggregates in concrete are of two types:

3

CONCRETE MIX DESIGN MANUAL

Coarse aggregates which refer to materials retained on 4.75mm sieve size; and Fine aggregates which are materials passing through 4.75mm sieve size. The proportion of fine aggregates to coarse aggregate in a concrete mix depend on the fineness of the fine aggregate, size/shape of coarse aggregates and the cement content. Details of the effect of properties of aggregates on properties of concrete mixes are presented in chapter three

1.7. Factors Affecting Concrete Mix Pro- portions The process of designing a concrete mix consists of selecting the appropriate proportions of cement, fine aggregate, coarse aggregate and water to produce concrete having specified properties. The most fundamental way of specifying mix proportions is in terms of the mass of material in a unit volume of fully compacted concrete. The various factors affecting the choice of mix proportions include:

1.7.1. Compressive Strength The compressive strength of concrete is the most universally used measure for concrete quality. It influences other properties of hardened concrete. Studies have shown that the compressive strength of concrete is inversely proportional to the water cement ratio within practical limit. The strength of the cement paste binder in concrete is dependent on the quality and quantity of the reaction of the paste components and the extent to which the hydration reaction has progressed. The strength of concrete increases with time as

long as there is sufficient hydration water/moisture at a favorable temperature. Hence, the strength at a particular age is dependent on both the original water- cement ratio as well as the degree to which the cementitious materials have hydrated. The mean compressive strength at a specific age, typically 28 days, determines the water- cement ratio of the mix. (Except in pozolanic cement where ages 56 to 90 days may be specified)

1.7.2. Workability The workability required for various types of construction is dependent on various factors. The Slump test is typically used to determine the degree of workability. For a given proportion of cement and aggregates, the higher the slump, the wetter the mixture and higher the workability.

1.7.3. Durability Typically, high strength concrete is generally more resistant to adverse conditions as compared to low strength concrete. However, in conditions where high strength is not required but the concrete would be exposed to adverse conditions, the durability requirement will determine the water-cement ratio to be used. See EN 206-1 Concrete - Part 1: Specification, performance, production and Conformity.

4

CONCRETE MIX DESIGN MANUAL

Coarse aggregates which refer to materials retained on 4.75mm sieve size; and Fine aggregates which are materials passing through 4.75mm sieve size. The proportion of fine aggregates to coarse aggregate in a concrete mix depend on the fineness of the fine aggregate, size/shape of coarse aggregates and the cement content. Details of the effect of properties of aggregates on properties of concrete mixes are presented in chapter three

1.7. Factors Affecting Concrete Mix Pro- portions The process of designing a concrete mix consists of selecting the appropriate proportions of cement, fine aggregate, coarse aggregate and water to produce concrete having specified properties. The most fundamental way of specifying mix proportions is in terms of the mass of material in a unit volume of fully compacted concrete. The various factors affecting the choice of mix proportions include:

1.7.1. Compressive Strength The compressive strength of concrete is the most universally used measure for concrete quality. It influences other properties of hardened concrete. Studies have shown that the compressive strength of concrete is inversely proportional to the water cement ratio within practical limit. The strength of the cement paste binder in concrete is dependent on the quality and quantity of the reaction of the paste components and the extent to which the hydration reaction has progressed. The strength of concrete increases with time as

long as there is sufficient hydration water/moisture at a favorable temperature. Hence, the strength at a particular age is dependent on both the original water- cement ratio as well as the degree to which the cementitious materials have hydrated. The mean compressive strength at a specific age, typically 28 days, determines the water- cement ratio of the mix. (Except in pozolanic cement where ages 56 to 90 days may be specified)

1.7.2. Workability The workability required for various types of construction is dependent on various factors. The Slump test is typically used to determine the degree of workability. For a given proportion of cement and aggregates, the higher the slump, the wetter the mixture and higher the workability.

1.7.3. Durability Typically, high strength concrete is generally more resistant to adverse conditions as compared to low strength concrete. However, in conditions where high strength is not required but the concrete would be exposed to adverse conditions, the durability requirement will determine the water-cement ratio to be used. See EN 206-1 Concrete - Part 1: Specification, performance, production and Conformity.

4

Cement - Part 1: Composition, specifications

and conformity criteria for common cements.

This standard defines 27 product in the family

of common cement that are grouped into 5

main types.

Nigeria are Portland Limestone Cements which

is in the CEM II class of cement as defined in

NIS 444-1. This cement composes of limestone

as a blended addition to clinker and gypsum.

The above table presents the following facts

that should be of interest to the user of

concrete products:

contain cement whose strength at 28days is

higher than that contained in a bag labeled

Grade 42.5 because of the overlap of the

strength of the two grades between 32.5MPa

and 42.5MPa. What one can then safely say is

that the cement in a Grade 32.5 bag has strength

of not less than 32.5MPa. Similarly, one can also

say that the cement in a Grade 42.5 bag has

strength of not less than 42.5MPa. This is

important in that those not familiar with this

fact could jump to the false conclusion that a

particular cement is substandard;

contain cement whose strength at 28days is

higher than that contained in a bag labeled

Grade 52.5 because of the overlap of the

strength of the two grades between 52.5MPa

and 62.5MPa. What one can then safely say is

that the cement in a Grade 42.5 bag has strength

of not less than 42.5MPa. Similarly, one can also

say that the cement in a Grade 52.5 bag has

strength of not less than 52.5MPa.

This is a very important issue to remember

when dealing with cements under this new

standard. It should therefore be noted that the

actual strength of cement in any bag can only be

determined by test – not from the label on the

bag. The label only guarantees minimum

strength, but a concrete mix design ensures the

use of the actual cement strength.

2.1.1. Strength Classes of Cement

The strength classes of cement (i.e 32.5 MPa or

42.5MPa) refer to the minimum strength of

cement mortar after 28 days curing and testing

as per standard conditions as specified in the

NIS 445:2003. The relationship between

compressive strength and water cement ratio

has been established as a set of curves for the

various strength classes of cement. Various

types and strength of classes of cements require

varying water contents to produce pastes of

standard consistency. Hence the water-cement

ratio required to achieve the target mean

strength is also dependent on the strength class

of cement. A higher strength

Part Two: Nigerian Cement, Aggregate, Admixture And Concrete Standards

32.5

32.5R

42.5

42.5R

52.5

52.5R

MM

Table 1 shows the strengths of various cements available in Nigeria.

5

Cement - Part 1: Composition, specifications

and conformity criteria for common cements.

This standard defines 27 product in the family

of common cement that are grouped into 5

main types.

Nigeria are Portland Limestone Cements which

is in the CEM II class of cement as defined in

NIS 444-1. This cement composes of limestone

as a blended addition to clinker and gypsum.

The above table presents the following facts

that should be of interest to the user of

concrete products:

contain cement whose strength at 28days is

higher than that contained in a bag labeled

Grade 42.5 because of the overlap of the

strength of the two grades between 32.5MPa

and 42.5MPa. What one can then safely say is

that the cement in a Grade 32.5 bag has strength

of not less than 32.5MPa. Similarly, one can also

say that the cement in a Grade 42.5 bag has

strength of not less than 42.5MPa. This is

important in that those not familiar with this

fact could jump to the false conclusion that a

particular cement is substandard;

contain cement whose strength at 28days is

higher than that contained in a bag labeled

Grade 52.5 because of the overlap of the

strength of the two grades between 52.5MPa

and 62.5MPa. What one can then safely say is

that the cement in a Grade 42.5 bag has strength

of not less than 42.5MPa. Similarly, one can also

say that the cement in a Grade 52.5 bag has

strength of not less than 52.5MPa.

This is a very important issue to remember

when dealing with cements under this new

standard. It should therefore be noted that the

actual strength of cement in any bag can only be

determined by test – not from the label on the

bag. The label only guarantees minimum

strength, but a concrete mix design ensures the

use of the actual cement strength.

2.1.1. Strength Classes of Cement

The strength classes of cement (i.e 32.5 MPa or

42.5MPa) refer to the minimum strength of

cement mortar after 28 days curing and testing

as per standard conditions as specified in the

NIS 445:2003. The relationship between

compressive strength and water cement ratio

has been established as a set of curves for the

various strength classes of cement. Various

types and strength of classes of cements require

varying water contents to produce pastes of

standard consistency. Hence the water-cement

ratio required to achieve the target mean

strength is also dependent on the strength class

of cement. A higher strength

Part Two: Nigerian Cement, Aggregate, Admixture And Concrete Standards

32.5

32.5R

42.5

42.5R

52.5

52.5R

MM

Table 1 shows the strengths of various cements available in Nigeria.

5

Based on the relationship between compressive

strength of concrete and the water to cement

ratio for the various cement classes, it can be

deduced that a lower water to cement ratio

would be required to produce a concrete of a

specific characteristic strength when using a

lower strength class of cement. That is to say, a

specified grade of concrete can be produced

using any strength class of cement provided the

mix design procedure is followed.

2.2. AGGREGATES Aggregates are the main constituents of concrete because they do not only give the body to the concrete, but they also have a significant effect on the properties of fresh and hardened concrete based on their shape, size, texture, grading and crushing value.

The overall mechanical property of concrete depends on certain properties of aggregates itself. These aggregate properties include the source of aggregates, size of aggregate, shape of aggregate, crushing type of aggregates, angularity index, surface texture, modulus of elasticity, bulk density, specific gravity, absorption and moisture content, grading of aggregates. For a good concrete mix, aggregates need to be clean, hard, and strong with the particles free of absorbed chemicals or coatings of clay and other fine materials that are likely to interfere with the process of hydration.

2.2.1. Types of Aggregates

Aggregate characteristics have a significant effect on the behavior of fresh and hardened p rope r t i e s o f conc r e t e . Ag g r eg a t e

characteristics are function of particle size and as such, the following classification is used in accordance to common practice: material retained in the No.4 sieve (4.75mm) is considered as coarse aggregate; material passing No.4 sieve (4.75mm) and retained in the No. 200 sieve (75μm) is considered as fine aggregate; and material passing No. 200 sieve is referred to as micro-fines.

2.2.2. Properties of Aggregates

The main characteristics of aggregate that affect the performance of fresh and hardened concrete, even though some variation in aggregate properties is expected, are as follows:

2.2.3. Shape and Texture The shape and texture of both coarse and fine aggregates play a significant role in the properties fresh and hardened concrete. The shape and texture of coarse aggregate play an important role on the behavior of fresh and hardened concrete as they affect the demand for fine aggregate.

Flaky and elongated particles should be limited to between 35 to 40 percent, or the shape coefficient determined by Equation 3.1 which should not be less than 0.20.

where is the volume of particle I

is the size of particle I

High voids, Poor Bond Grip, Bleeding.

Good Bond Grip

Increase segregation, Finishing

Elongated

Rough

Water Demand.

Table 3: Impact of aggregates shape and texture in concrete.

Properties

Influence on Concrete Performance

Bonding, Water Demand, Absorption

Cohension, Water Demand (Strength)

Table 2: Aggregate properties and its influence on concrete performance.

Strength, Water demand

Based on the relationship between compressive

strength of concrete and the water to cement

ratio for the various cement classes, it can be

deduced that a lower water to cement ratio

would be required to produce a concrete of a

specific characteristic strength when using a

lower strength class of cement. That is to say, a

specified grade of concrete can be produced

using any strength class of cement provided the

mix design procedure is followed.

2.2. AGGREGATES Aggregates are the main constituents of concrete because they do not only give the body to the concrete, but they also have a significant effect on the properties of fresh and hardened concrete based on their shape, size, texture, grading and crushing value.

The overall mechanical property of concrete depends on certain properties of aggregates itself. These aggregate properties include the source of aggregates, size of aggregate, shape of aggregate, crushing type of aggregates, angularity index, surface texture, modulus of elasticity, bulk density, specific gravity, absorption and moisture content, grading of aggregates. For a good concrete mix, aggregates need to be clean, hard, and strong with the particles free of absorbed chemicals or coatings of clay and other fine materials that are likely to interfere with the process of hydration.

2.2.1. Types of Aggregates

Aggregate characteristics have a significant effect on the behavior of fresh and hardened p rope r t i e s o f conc r e t e . Ag g r eg a t e

characteristics are function of particle size and as such, the following classification is used in accordance to common practice: material retained in the No.4 sieve (4.75mm) is considered as coarse aggregate; material passing No.4 sieve (4.75mm) and retained in the No. 200 sieve (75μm) is considered as fine aggregate; and material passing No. 200 sieve is referred to as micro-fines.

2.2.2. Properties of Aggregates

The main characteristics of aggregate that affect the performance of fresh and hardened concrete, even though some variation in aggregate properties is expected, are as follows:

2.2.3. Shape and Texture The shape and texture of both coarse and fine aggregates play a significant role in the properties fresh and hardened concrete. The shape and texture of coarse aggregate play an important role on the behavior of fresh and hardened concrete as they affect the demand for fine aggregate.

Flaky and elongated particles should be limited to between 35 to 40 percent, or the shape coefficient determined by Equation 3.1 which should not be less than 0.20.

where is the volume of particle I

is the size of particle I

High voids, Poor Bond Grip, Bleeding.

Good Bond Grip

Increase segregation, Finishing

Elongated

Rough

Water Demand.

Table 3: Impact of aggregates shape and texture in concrete.

Properties

Influence on Concrete Performance

Bonding, Water Demand, Absorption

Cohension, Water Demand (Strength)

Table 2: Aggregate properties and its influence on concrete performance.

Strength, Water demand

CONCRETE MIX DESIGN MANUAL

2.2.4. Maximum Size of Aggregate Maximum size of aggregate, MSA, influences workabil ity, strength, shrinkage, and permeability. Mixtures with large maximum size of coarse aggregate tend to produce concrete with better workability, probably because of the decrease in specific surface. There is an optimal maximum size of coarse aggregate that produces the highest strength for a given consistency and cement content. In high- performance concrete (HPC) with low water- cement ratio and high cement content, a high value of MSA tends to reduce strength. This can be explained by the observation that bond with large particles tends to be weaker than with small particles due to smaller surface area-to- volume ratios. Mixtures with coarse aggregates having large maximum size tends to have reduced shrinkage and creep. Finally, for a given water-cement ratio, the permeability increases as the maximum size of the aggregate increases.

2.2.5. Limit on Deleterious Matter. In natural sands, deleterious particles like clay minerals and organic matter, mostly present in the minus 63μm portion, increase significantly the demand for water. It is recommended that the limit of 5% passing 63μm be adopted for use in concrete mix design.

2.2.6. Aggregates in Nigerian Construc- tion Industry The aggregates commonly available in the Nigerian construction industry are the fine aggregates [sharp sand and stone dust] and coarse aggregates [natural gravel and crushed rock]. In selecting aggregates for use in concrete, the grading curve for such an

aggregate is an important parameter for determining its suitability for use.

EN 12620 Aggregate for Concrete provides

grading limits within which suitable aggregates

are expected to lie.

The maximum size of coarse aggregate is the

standard sieve size through which at least 90%

of the coarse aggregates would pass. Typical

maximum sizes of aggregate in use in Nigeria

are 40mm, 20mm and 10mm with 20mm being

the most common. The maximum size of

aggregate affects the workability and strength

of the concrete. It also affects the required

water content for a certain workability and fine

aggregate content required for achieving a

cohesive mix.

1 2

.......... 3.1

[ ....... ] 6

n

n

1 2 3 4 5 6

LOWER LIMIT FOR 20MM 10 - 15MM AGGREGATE

LOWER LIMIT FOR 20MM 5-15MM AGGREGATE UPPER LIMIT FOR 20MM

100

90

80

70

60

50

40

30

20

10

0

Fig. 2 - Grading curve for 5-15 coarse aggregate

SIEVE NO

CONCRETE MIX DESIGN MANUAL

2.2.4. Maximum Size of Aggregate Maximum size of aggregate, MSA, influences workabil ity, strength, shrinkage, and permeability. Mixtures with large maximum size of coarse aggregate tend to produce concrete with better workability, probably because of the decrease in specific surface. There is an optimal maximum size of coarse aggregate that produces the highest strength for a given consistency and cement content. In high- performance concrete (HPC) with low water- cement ratio and high cement content, a high value of MSA tends to reduce strength. This can be explained by the observation that bond with large particles tends to be weaker than with small particles due to smaller surface area-to- volume ratios. Mixtures with coarse aggregates having large maximum size tends to have reduced shrinkage and creep. Finally, for a given water-cement ratio, the permeability increases as the maximum size of the aggregate increases.

2.2.5. Limit on Deleterious Matter. In natural sands, deleterious particles like clay minerals and organic matter, mostly present in the minus 63μm portion, increase significantly the demand for water. It is recommended that the limit of 5% passing 63μm be adopted for use in concrete mix design.

2.2.6. Aggregates in Nigerian Construc- tion Industry The aggregates commonly available in the Nigerian construction industry are the fine aggregates [sharp sand and stone dust] and coarse aggregates [natural gravel and crushed rock]. In selecting aggregates for use in concrete, the grading curve for such an

aggregate is an important parameter for determining its suitability for use.

EN 12620 Aggregate for Concrete provides

grading limits within which suitable aggregates

are expected to lie.

The maximum size of coarse aggregate is the

standard sieve size through which at least 90%

of the coarse aggregates would pass. Typical

maximum sizes of aggregate in use in Nigeria

are 40mm, 20mm and 10mm with 20mm being

the most common. The maximum size of

aggregate affects the workability and strength

of the concrete. It also affects the required

water content for a certain workability and fine

aggregate content required for achieving a

cohesive mix.

1 2

.......... 3.1

[ ....... ] 6

n

n

1 2 3 4 5 6

LOWER LIMIT FOR 20MM 10 - 15MM AGGREGATE

LOWER LIMIT FOR 20MM 5-15MM AGGREGATE UPPER LIMIT FOR 20MM

100

90

80

70

60

50

40

30

20

10

0

Fig. 2 - Grading curve for 5-15 coarse aggregate

SIEVE NO

7

The larger the size of the maximum aggregate, the lower the surface area of the coarse aggregates. With a higher surface area, a higher water content is required to coat the particles and develop workability. Also, a higher maximum size of aggregate would require a lower fine aggregate content to coat the particles and maintain cohesiveness of the concrete mix. This implies that for the same workability, coarse aggregate with maximum size of 40mm would require a lower water cement ratio and thus higher strength compared to coarse aggregate with maximum size of 20mm. However, maximum size of aggregate is restricted by the clear cover and the minimum distance between reinforcement bars. See EN 12620 Aggregates for Concrete.

2.2.8. Grading and Type of Aggregate

Typically, aggregates can be single sized or graded in terms of particle size distribution. The grading of aggregate is significant in achieving a dense and cohesive concrete mix. The voids created by the larger coarse aggregates are filled by the smaller coarse aggregates and hence, the volume of cement-sand-water paste required to fill the final voids is minimum. By proper grading of coarse aggregate, the compactibility of concrete is improved and segregation is minimized especially for higher workability.

The type and source of aggregate also has a

significant effect on the compressive strength

of concrete. Typical aggregates in use in Nigeria

can be categorized in the crushed and

uncrushed classes. It is widely accepted that

concrete produced from crushed aggregate has

a higher strength compared to concrete

produced from uncrushed aggregates. This can

be attributed to the rough surface texture of the

crushed aggregates which gives it a better

bonding with the cement gel. The grading of

aggregate is significant in attaining an

economical mix as it affects the amount of concrete that can be obtained with a given amount of cement and water.

2.3. ADMIXTURES Admixtures are constituent materials other than Portland cement, aggregate and water added to concrete mixture before or during mixing to modify one or more characteristic of concrete either in the wet or hardened state. Admixtures can be group into two major group as Mineral admixtures and Chemical Admixtures.

2.3.1. Mineral Admixtures Mineral admixtures are either naturally occurring or as by-product of industrial processes. They are known as supplementary cementing materials, which could be blended with clinker to produce blended or composite cement as specified in NIS 444-1 Mineral admixture could also be added during production of cement to alter characteristic performance of concrete.

2.3.1.1. Types of Mineral Admixtures

Ÿ Ground Granulated Blast Furnace Slag

Ÿ Fly Ash (Siliceous or Calcareous)

Ÿ Silica Fume

are the result of controlled calcination

of rice husk and kaolinite clay falls

under the calcined pozolana etc.

2.3.2. Chemical Admixtures

added to concrete to alter the characteristic

either at the wet or hardened state. The

composition and the performance criteria are

listed in EN 934-2 Admixtures for Concrete

Mortar and Grout.

CONCRETE MIX DESIGN MANUAL

The larger the size of the maximum aggregate, the lower the surface area of the coarse aggregates. With a higher surface area, a higher water content is required to coat the particles and develop workability. Also, a higher maximum size of aggregate would require a lower fine aggregate content to coat the particles and maintain cohesiveness of the concrete mix. This implies that for the same workability, coarse aggregate with maximum size of 40mm would require a lower water cement ratio and thus higher strength compared to coarse aggregate with maximum size of 20mm. However, maximum size of aggregate is restricted by the clear cover and the minimum distance between reinforcement bars. See EN 12620 Aggregates for Concrete.

2.2.8. Grading and Type of Aggregate

Typically, aggregates can be single sized or graded in terms of particle size distribution. The grading of aggregate is significant in achieving a dense and cohesive concrete mix. The voids created by the larger coarse aggregates are filled by the smaller coarse aggregates and hence, the volume of cement-sand-water paste required to fill the final voids is minimum. By proper grading of coarse aggregate, the compactibility of concrete is improved and segregation is minimized especially for higher workability.

The type and source of aggregate also has a

significant effect on the compressive strength

of concrete. Typical aggregates in use in Nigeria

can be categorized in the crushed and

uncrushed classes. It is widely accepted that

concrete produced from crushed aggregate has

a higher strength compared to concrete

produced from uncrushed aggregates. This can

be attributed to the rough surface texture of the

crushed aggregates which gives it a better

bonding with the cement gel. The grading of

aggregate is significant in attaining an

economical mix as it affects the amount of concrete that can be obtained with a given amount of cement and water.

2.3. ADMIXTURES Admixtures are constituent materials other than Portland cement, aggregate and water added to concrete mixture before or during mixing to modify one or more characteristic of concrete either in the wet or hardened state. Admixtures can be group into two major group as Mineral admixtures and Chemical Admixtures.

2.3.1. Mineral Admixtures Mineral admixtures are either naturally occurring or as by-product of industrial processes. They are known as supplementary cementing materials, which could be blended with clinker to produce blended or composite cement as specified in NIS 444-1 Mineral admixture could also be added during production of cement to alter characteristic performance of concrete.

2.3.1.1. Types of Mineral Admixtures

Ÿ Ground Granulated Blast Furnace Slag

Ÿ Fly Ash (Siliceous or Calcareous)

Ÿ Silica Fume

are the result of controlled calcination

of rice husk and kaolinite clay falls

under the calcined pozolana etc.

2.3.2. Chemical Admixtures

added to concrete to alter the characteristic

either at the wet or hardened state. The

composition and the performance criteria are

listed in EN 934-2 Admixtures for Concrete

Mortar and Grout.

CONCRETE MIX DESIGN MANUAL

2.3.2.1. T y p e s o f C h e m i c a l Admixtures Ÿ Water reducing/Plasticizing Ÿ High-range water reducing/super-

plasticizing Ÿ Water retaining (Reduces Bleeding) Ÿ Water resisting (for Waterproofing) Ÿ Air Entraining Ÿ Set Retarding Ÿ Set Accelerating Ÿ Hardening Accelerating

Others are; Ÿ Set retarding/water reducing/

plasticizing. Ÿ Set retarding/high-range water

reducing/super-plasticizing. Ÿ Set Accelerating/water reducing/

plasticizing.

Admixture could be used singularly or in combinations to attain any desired performance effect in concrete.

2.4. CONCRETE GRADES Concrete is generally designed in grades which, in Nigeria, correspond to classes of strength and therefore categories of concrete below those shown in the Table 5 should never be used. Consequently, the single most important deleterious effect on building strength and durability is poor concreting. The concrete should be 'designed' OR 'designated'. In a 'designated concrete', the producer who is generally the constructor (not necessarily the same as a contractor) is required to produce a material to satisfy

the designated strength and consistency (workability) using a particular aggregate s ize. Designated concretes are designated as Grade 30, for example, based on the cube strength up to Grade 50, according to the application involved. A designed concrete, on the other hand, is the one whose strength class, cement type, and limits to composition including water/cement ratio, cement content (mix ratio) are specified.

The symbol f generally denotes ck

characteristic strength based on cylinder strength of the concrete. The term f denotes cube strength.cu

Prestressed & Reinforced concrete subject to chlorides

30C30/37 37

Minimum Characteristic

Cylinder Strength

Minimum Characteristic

Cube Strength

Table 4: Strength Classes of Concrete according to EN 206-1

9

Ÿ Water reducing/Plasticizing

Ÿ Air Entraining

Ÿ Set Retarding

Ÿ Set Accelerating

Ÿ Hardening Accelerating

Ÿ Set retarding/water reducing/ plasticizing.

Ÿ S e t r e t a rd i n g / h i g h - r a n g e wa t e r

reducing/super-plasticizing.

plasticizing.

combinations to attain any desired performance

effect in concrete.

2.4. CONCRETE GRADES

and therefore categories of concrete below

those shown in the Table 5 should never be

used. Consequently, the single most important

deleterious effect on building strength and

durability is poor concreting. The concrete

should be 'designed' OR 'designated'. In a

'designated concrete', the producer who is

generally the constructor (not necessarily the

same as a contractor) is required to produce a

material to satisfy the designated strength and

consistency (workability) using a particular

aggregate size. Designated concretes are

designated as Grade 30, for example, based on

the cube strength up to Grade 50, according to

the application involved. A designed concrete,

on the other hand, is the one whose strength

class, cement type, and limits to composition including water/cement ratio, cement content (mix ratio) are specified.

The symbol f genera l ly denotes c k

characteristic strength based on cylinder

strength of the concrete. The term f denotes cu

cube strength.

30C30/37 37

Minimum Characteristic

Cylinder Strength

Minimum Characteristic

Cube Strength

Table 4: Strength Classes of Concrete according to EN 206-1

9

CONCRETE MIX DESIGN MANUAL

3.1. Introduction to mix design For ease of calculation, the mix design procedure is divided into five stages. Each step by step procedure deals with a particular aspect and ends with an important parameter. The step by step procedure is as follows:

Step 1: Determination of target mean strength Step 2: Determination of Water-cement ratio Step 3: Determination of water content Step4: Determination of cement content Step5: Determination of aggregate content

3.2. Determination of Target Mean Strength

As a result of the variability of concrete in production, it is necessary to design the mix to have a mean strength greater than the specified characteristic strength. Hence, the target compressive strength is obtained from the equation:

where f = the target mean strengthm

f = the specified characteristic c strength k = a constant (taken as 1.64 for a 5% defective level) s = standard deviation

Typically, the standard deviation is obtained from the field by carrying out tests on a minimum of 20-30 samples taken from the site as early as possible. In cases of significant changes in production of concrete batches, the standard deviation value should be calculated for new batches. The standard deviation recommended in this manual is 6MPa. Where however a producer is able to achieve lesser value, he can use his own value.

3.3. Determination of Water- Cement ratio

Different cements and aggregates of various maximum size, grading and other characteristics may produce concretes of different compressive strengths at the same water-cement ratio. Hence, the relationship between strength and water cement ratio should be established for the materials to be used. If this is not available, the free water-cement ratio corresponding to the target strength may be obtained from Fig. 4.1 The water cement ratio selected should be checked against the maximum water cement ratio for the requirements of durability and the lower of the two values is recommended.

PART THREE: MIX DESIGN PROCEDURE

10

For ease of calculation, the mix design

procedure is divided into five stages. Each step

by step procedure deals with a particular aspect

and ends with an important parameter. The

step by step procedure is as follows:

Step 1: Determination of target mean strength

Step 2: Determination of Water-cement ratio

Step 3: Determination of water content

Step4: Determination of cement content

Step5: Determination of aggregate content

3.2. Determination of Target Mean

Strength

have a mean strength greater than the specified

characteristic strength. Hence, the target

compressive strength is obtained from the

equation:

where f = the target mean strengthm

f = the specified characteristic c strength k = a constant (taken as 1.64 for a 5% defective level) s = standard deviation

Typically, the standard deviation is obtained from the field by carrying out tests on a minimum of 20-30 samples taken from the site as early as possible. In cases of significant changes in production of concrete batches, the standard deviation value should be calculated for new batches. The standard deviation recommended in this manual is 6MPa. Where however a producer is able to achieve lesser value, he can use his own value.

3.3. Determination of Water-Cement ratio

Different cements and aggregates of various max imum s i ze , g rad ing and o ther characteristics may produce concretes of different compressive strengths at the same water-cement ratio. Hence, the relationship between strength and water cement ratio should be established for the materials to be used. If this is not available, the free water- cement ratio corresponding to the target strength may be obtained from Fig. 4.1 The water cement ratio selected should be checked against the maximum water cement ratio for the requirements of durability and the lower of the two values is recommended.

PART THREE: MIX DESIGN PROCEDURE

10

CONCRETE MIX DESIGN MANUAL

Alternatively, the equation of the strength versus water/cement graph for Grade 32.5 cement is for [ ]

Where is the target mean strength of the mix; r is the water/cement ratio From equation 4.1, we have:

The equation of the strength versus water/cement graph for Grade 42.5 cement is[for]:

Where is the target mean strength of the mix; r is the water/cement ratio From equation 4.3, we have:

It should be noted here that the procedure adopted limits the target mean strength for concrete using Grade 32.5 cement to 44MPa while that of Grade 42.5 cement is limited to 57MPa for water/cement ratios between 0.3 and 0.9.

It should be noted here that the procedure adopted limits the target mean strength for concrete using Grade 32.5 cement to 52MPa while that of Grade 42.5 cement is limited to 68MPa.

3.4. Determination of Water content The water content of concrete is dependent on the type and maximum size of concrete to give a specified workability. The ranges of slump covered in this manual are 30 to 60mm and 60 to 180mm. Maximum aggregate sizes are also limited to 20 and 40mm. The recommended water content are as shown on Table 4.1.

3.5. Determination of cement content The cement content is determined from the water-cement ratio and the quantity of water.

The resulting value should be checked against the maximum and minimum value specified If the specified maximum cement content is exceeded, a higher cement grade should be used to enable the producer meet this requirement. Alternatively, super plasticizers could be used to meet other requirement at the determined cement content. If the minimum cement content is higher that the earlier calculated value, this minimum value should be adopted and the water content should be recalculated to provide the same water/cement ratio at the specified minimum cement content.

3.6. Determination of aggregate content To determine the total aggregate content, an estimate of the density of the fully compacted concrete should be known. From tests carried out, a density value of 2400kg/m3 is recommended for use for all mixes using normal weight aggregates. The total aggregate is obtained from the relationship:

The fine and coarse aggregate content are

determined by obtaining the proportion of fine

aggregate in the total aggregate content. Due to

the fact that many coarse aggregates

Table 4. : Approximate Free water contents required to give various levels

of workability

6 4 6 2 . . . . . . . . . . [ 5 . 1 ]rs = - +

6 2 .. . .. . . .. . .[ 5 . 2 ]

8 3 .. . .. . . .. . .[ 5 . 4 ]

s- =

12

Alternatively, the equation of the strength versus water/cement graph for Grade 32.5 cement is for [ ]

Where is the target mean strength of the mix; r is the water/cement ratio From equation 4.1, we have:

The equation of the strength versus water/cement graph for Grade 42.5 cement is[for]:

Where is the target mean strength of the mix; r is the water/cement ratio From equation 4.3, we have:

It should be noted here that the procedure adopted limits the target mean strength for concrete using Grade 32.5 cement to 44MPa while that of Grade 42.5 cement is limited to 57MPa for water/cement ratios between 0.3 and 0.9.

It should be noted here that the procedure adopted limits the target mean strength for concrete using Grade 32.5 cement to 52MPa while that of Grade 42.5 cement is limited to 68MPa.

3.4. Determination of Water content The water content of concrete is dependent on the type and maximum size of concrete to give a specified workability. The ranges of slump covered in this manual are 30 to 60mm and 60 to 180mm. Maximum aggregate sizes are also limited to 20 and 40mm. The recommended water content are as shown on Table 4.1.

3.5. Determination of cement content The cement content is determined from the water-cement ratio and the quantity of water.

The resulting value should be checked against the maximum and minimum value specified If the specified maximum cement content is exceeded, a higher cement grade should be used to enable the producer meet this requirement. Alternatively, super plasticizers could be used to meet other requirement at the determined cement content. If the minimum cement content is higher that the earlier calculated value, this minimum value should be adopted and the water content should be recalculated to provide the same water/cement ratio at the specified minimum cement content.

3.6. Determination of aggregate content To determine the total aggregate content, an estimate of the density of the fully compacted concrete should be known. From tests carried out, a density value of 2400kg/m3 is recommended for use for all mixes using normal weight aggregates. The total aggregate is obtained from the relationship:

The fine and coarse aggregate content are

determined by obtaining the proportion of fine

aggregate in the total aggregate content. Due to

the fact that many coarse aggregates

Table 4. : Approximate Free water contents required to give various levels

of workability

6 4 6 2 . . . . . . . . . . [ 5 . 1 ]rs = - +

6 2 .. . .. . . .. . .[ 5 . 2 ]

8 3 .. . .. . . .. . .[ 5 . 4 ]

s- =

12

available from the quarries in Nigeria do not fit into the BS882 envelopes for coarse aggregates, the use of combined aggregate grading envelope is recommended. Two methods are recommended for determining the proportion of fine aggregates in the concrete.

The first involves plotting the grading curves of

the fine and coarse aggregates on the same axis

on the graph paper and determining the

percentage combinations of the two aggregates

which gives a grading very close to the median

of the BS882 envelope.

software developed by Professor Charles

Uko of the University of Uyo, Uyo, Nigeria

which automatically determines the most

suitable combination once values of

percentages passing different sieve sizes

are provided for the two aggregates.

The fine aggregate and coarse aggregate

contents are calculated from the relationships

3.7. Trial Mixes

checked using trial batches. The workability of

the first trial mix should be measured and if it's

different from the stipulated value, the water

content should be adjusted suitably. With the

adjusted water content, the mix design should

be recalculated with the original water-cement

ratio. Two more trial mixes should be made with

this adjusted water content but at varying water

cement ratios of ±10% of the original value.

The last three mixes provide sufficient

information on the relationship between

compressive strength and water-cement ratio.

This can be used to carry out mix proportions

for field trials using actual methods of concrete

production on site.

The issue of trial mix must be taken very seriously in view of the variables involved in

CONCRETE MIX DESIGN MANUAL

1 2 3 4 5 6 7 8 9 10

FINE SAND % PASSING 5-15 AGG% PASSING Bs882 ALL-IN MEAN

POINT A = 45%

POINT B =24%

G

Fig. 4.2 - Combined aggregate curves for fine sand and 5-15 coarse aggregate

POINT A = 45%

POINT B=17%

1 2 3 4 5 6 7 8 9 10

POINT A = 45%

POINT B =17%

Fig. 4.3 - Combined aggregate curves for fine sand and 10-15 coarse aggregate

Fig. 4.5 - Combined aggregate grading curve for 21% fines and 79% coarse SIEVE NO

1 2 3 4 5 6 7 8 9 10

LOWER LIMIT FOR 20MM UPPER LIMIT FOR 20MM COMB AGG [21:79]

[USING COMBAG 16]

G

100

90

80

70

60

50

40

30

20

10

0

100

90

80

70

60

50

40

30

20

10

0

Fig. 4.4 - Combined aggregate grading curve for 21% fines and 79% coarse

1 2 3 4 5 6 7 8 9 10

LOWER LIMIT FOR 20MM UPPER LIMIT FOR 20MM COMB AGG [21:79]

SIEVE NO

P E

R C

E N

TA G

E P

A S

S IN

G

13

available from the quarries in Nigeria do not fit into the BS882 envelopes for coarse aggregates, the use of combined aggregate grading envelope is recommended. Two methods are recommended for determining the proportion of fine aggregates in the concrete.

The first involves plotting the grading curves of

the fine and coarse aggregates on the same axis

on the graph paper and determining the

percentage combinations of the two aggregates

which gives a grading very close to the median

of the BS882 envelope.

software developed by Professor Charles

Uko of the University of Uyo, Uyo, Nigeria

which automatically determines the most

suitable combination once values of

percentages passing different sieve sizes

are provided for the two aggregates.

The fine aggregate and coarse aggregate

contents are calculated from the relationships

3.7. Trial Mixes

checked using trial batches. The workability of

the first trial mix should be measured and if it's

different from the stipulated value, the water

content should be adjusted suitably. With the

adjusted water content, the mix design should

be recalculated with the original water-cement

ratio. Two more trial mixes should be made with

this adjusted water content but at varying water

cement ratios of ±10% of the original value.

The last three mixes provide sufficient

information on the relationship between

compressive strength and water-cement ratio.

This can be used to carry out mix proportions

for field trials using actual methods of concrete

production on site.

The issue of trial mix must be taken very seriously in view of the variables involved in

POINT A = 45%

1 2 3 4 5 6 7 8 9 10

FINE SAND % PASSING 5-15 AGG% PASSING Bs882 ALL-IN MEAN

POINT A = 45%

POINT B =24%

G

Fig. 4.2 - Combined aggregate curves for fine sand and 5-15 coarse aggregate

100

90

80

70

60

50

40

30

20

10

0

1 2 3 4 5 6 7 8 9 10

POINT B =17%

Fig. 4.3 - Combined aggregate curves for fine sand and 10-15 coarse aggregate

Fig. 4.5 - Combined aggregate grading curve for 21% fines and 79% coarse SIEVE NO

1 2 3 4 5 6 7 8 9 10

LOWER LIMIT FOR 20MM UPPER LIMIT FOR 20MM COMB AGG [21:79]

[USING COMBAG 16]

G

100

90

80

70

60

50

40

30

20

10

0

100

90

80

70

60

50

40

30

20

10

0

Fig. 4.4 - Combined aggregate grading curve for 21% fines and 79% coarse

1 2 3 4 5 6 7 8 9 10

LOWER LIMIT FOR 20MM UPPER LIMIT FOR 20MM COMB AGG [21:79]

SIEVE NO

P E

R C

E N

TA G

E P

A S

S IN

concrete production.

WORKED EXAMPLES This example involves the design of a concrete mix using Grade 32.5 cement and river sand as fine aggregate. The coarse aggregate is 10-15mm crushed rock with sieve analysis already done and as shown on Fig.

15

the design of grade 30 concrete, using both

grade 32.5 cement and grade 42.5 cements

respectively. the coarse aggregate was crushed

rock with maximum aggregate size 20mm.

Fine aggregate was sharp sand and the

percentage fines used was determined after

sieve analysis and combination of aggregate

using the method recommended or the

software COMBA (see Fig. 5)

15

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

1

1.1

1.2

1.3

1.4

1.5

1.6

1.7

1.8

19

2

2.1

2.2

2.3

3

3.1

3.2

3.3

3.4

4

4.1

4.2

5

5.1

5.2

5.3

5.4

6

6.1

6.2

6.3

6.4

MIX DESIGN EXAMPLE FOR GRADE 30 CONCRETE [USING GRADE 32.5 CEMENT]

S/NO ITEM UNITS

20

225

NONE

30

4

6.56

36.56

32.5

0.40

Crushed

Uncrushed

STAGE 6 - Trial Mix Quantities Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

100mm cube 150mm cube

2.8 7.1 7.0 13.1

5.6 14.2 14.1 26.1

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

1

1.1

1.2

1.3

1.4

1.5

1.6

1.7

1.8

19

2

2.1

2.2

2.3

3

3.1

3.2

3.3

3.4

4

4.1

4.2

5

5.1

5.2

5.3

5.4

6

6.1

6.2

6.3

6.4

MIX DESIGN EXAMPLE FOR GRADE 30 CONCRETE [USING GRADE 32.5 CEMENT]

S/NO ITEM UNITS

20

235

NONE

30

4

6.56

36.56

32.5

0.40

Crushed

Uncrushed

STAGE 6 - Trial Mix Quantities Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

100mm cube 150mm cube

2.9 7.4 6.9 12.8

5.9 14.8 13.8 25.6

CONCRETE MIX DESIGN MANUAL

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

1

1.1

1.2

1.3

1.4

1.5

1.6

1.7

1.8

19

2

2.1

2.2

2.3

3

3.1

3.2

3.3

3.4

4

4.1

4.2

5

5.1

5.2

5.3

5.4

6

6.1

6.2

6.3

6.4

MIX DESIGN EXAMPLE FOR GRADE 30 CONCRETE [USING GRADE 42.5 CEMENT]

S/NO ITEM UNITS

20

225

NONE

30

4

6.56

36.56

42.5

0.55

Crushed

Uncrushed

STAGE 6 - Trial Mix Quantities Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

100mm cube 150mm cube

2.8 5.1 7.7 14.4

CONCRETE MIX DESIGN MANUAL

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

1

1.1

1.2

1.3

1.4

1.5

1.6

1.7

1.8

19

2

2.1

2.2

2.3

3

3.1

3.2

3.3

3.4

4

4.1

4.2

5

5.1

5.2

5.3

5.4

6

6.1

6.2

6.3

6.4

MIX DESIGN EXAMPLE FOR GRADE 30 CONCRETE [USING GRADE 42.5 CEMENT]

S/NO ITEM UNITS

20

235

NONE

30

4

6.56

36.56

42.5

0.55

Crushed

Uncrushed

STAGE 6 - Trial Mix Quantities Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

100mm cube 150mm cube

2.9 5.3 7.6 14.1

5.9 10.6 15.2 28.3

CONCRETE MIX DESIGN MANUAL

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

S/NO ITEM UNITS

Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

STAGE 6 - Trial Mix Quantities 100mm cube 150mm cube

18

Cement Content Maximum cement content [specified] Minimum cement content [specified] Modified free-water/cement ratio

Concrete density Total aggregate content STAGE 5

Grading of fine aggregate

Proportion of fine aggregate [%]

S/NO ITEM UNITS

Water [kg] Cement [kg] Fine aggregate [kg] Coarse aggregate [kg]

STAGE 6 - Trial Mix Quantities 100mm cube 150mm cube

18

The following important points should

be noted when carrying out a mix design: 1. All cement brands to be used must be clearly labeled indicating the strength class 2. A site trial mix design should be carried out to ensure the suitability of the mix on site. Cubes should be cast during the trial and should be tested pr ior to the commencement of concreting works 3. Concrete mix design procedure assumes that aggregates are in the saturated surface dry condition. Hence, coarse aggregates should be wetted before use to bring them to this condition 4. Water cement ratio must be strictly controlled on the site as it governs the strength and workabil i ty of the concrete. 5. Ensure cement is stocked properly in a waterproof area and is not in direct contact with floor or walls 6. Cubes should always be cast for every batch of concrete. Ensure that a minimum o f t h r e e c u b e s a r e produced for 28days testing. 7. The following are essentials for a site laboratory:

· Set of 12 cube moulds of size

150mm

scale

25mm, 20mm, 12.5mm, 10mm,

and 4.75mm, 2.36mm, 1.18mm,

a pan and lid.

site, a suitable one should be identified

close to the site.

CONCRETE MIX DESIGN MANUAL

RECOMMENDATIONS The following important points should be noted when carrying out a mix design: 1. All cement brands to be used must be clearly labeled indicating the strength class 2. A site trial mix design should be carried out to ensure the suitability of the mix on site. Cubes should be cast during the trial and should be tested p r i o r t o t h e commencement of c o n c r e t i n g works 3. Concrete mix des ign procedure assumes that aggregates are in the saturated surface dry condition. Hence, coarse aggregates should be wetted before use to bring them to this condition 4. Water cement ratio must be strictly controlled on the site as it governs the s t r e n g t h a n d wo r k a b i l i t y o f t h e concrete. 5. Ensure cement is stocked properly in a waterproof area and is not in direct contact with floor or walls 6. Cubes should always be cast for every batch of concrete. Ensure that a minimum of three cubes are produced for 28days testing. 7. The following are essentials for a site laboratory:

· Set of 12 cube moulds of size

150mm

scale

25mm, 20mm, 12.5mm, 10mm,

and 4.75mm, 2.36mm, 1.18mm,

a pan and lid.

site, a suitable one should be identified close to

the site.

A.1. TESTING FRESH CONCR- ETE (SLUMP TEST) PROC- EDURE

A.1.1. Apparatus. · Slump cone · Base plate. · Compacting rod · Funnel · Ruler · Scoop · Timer · Shovel · Moist cloth

A.1.2. Testing Procedure · Mix or remix the concrete sample

thoroughly. · Dampen the inside of the slump cone,

the funnel and the base plate by wiping with a damp cloth.

· Clamp the slump cone to the base plate or stand firmly on the foot pieces to hold the slump down and in place.

· Fill the slump cone in 3 equal layer compacting each layer with 25 stroke of the tamping rod, distributing the strokes uniformly all over the surface of the layer. Repeat this for the second and the third layer tampering each layer through to the surface of the underlining layer.

· After compacting the third layer remove the funnel and strike off any excess concrete by means of sawing and the rolling motion of the tampering rod.

· Remove spilled concrete from the base plate and around the slump cone.

· Remove the slump cone by raising it vertically in a gentle manner within 5 to

10 seconds. · The operation from filling to the

remover of the slump cone should be done within 150 seconds.

· Immediately after the removal of the slump cone, measure and record the slump as the difference between the highest point on the concrete and the height of the slump cone to the nearest 10mm.

The result is valid only if the specimen yields a true slump. See EN 12350-2 Testing fresh concrete. Slump-test for more detail.

A . 2 . T E S T I N G H A R D E N E D CONCRETE (COMPRESSIVE TEST) PROCEDURE A.2.1. Sample Preparation

· Wipe the excess moisture on the test

specimen with a clean towel

· Wipe the surface of the platen on the

testing machine clean of any particle

especially from previous tests.

auxiliary platen or spacing blocks

between the specimen and the platens

of the testing machine.

so that the load is applied on the

smooth surfaces and not on the trowel

surface.

with the center of the upper and the

lower platen of the testing machine.

20

APPENDIX

A.1. TESTING FRESH CONCR- E T E ( S L U M P T E S T ) P R O C - EDURE

A.1.1. Apparatus. · Slump cone · Base plate. · Compacting rod · Funnel · Ruler · Scoop · Timer · Shovel · Moist cloth

A.1.2. Testing Procedure · Mix or remix the concrete sample

thoroughly. · Dampen the inside of the slump cone,

the funnel and the base plate by wip